5KHRORJ\ 7KHRU\DQG$SSOLFDWLRQV

TAINSTRUMENTS.COM &RXUVH2XWOLQH

Basics in Rheology Theory Oscillation TA Rheometers Linear Viscoelasticity Instrumentation Setting up Oscillation Tests Choosing a Geometry Transient Testing Calibrations Applications of Rheology Flow Tests Polymers Viscosity Structured Fluids Setting up Flow Tests Advanced Accessories

TAINSTRUMENTS.COM %DVLFVLQ5KHRORJ\7KHRU\

TAINSTRUMENTS.COM 5KHRORJ\$Q,QWURGXFWLRQ

Rheology: The study of stress-deformation relationships

TAINSTRUMENTS.COM 5KHRORJ\$Q,QWURGXFWLRQ

Rheology is the science of flow and deformation of matter The word ‘Rheology’ was coined in the 1920s by Professor E C Bingham at Lafayette College in Indiana Flow is a special case of deformation The relationship between stress and deformation is a property of the material

ୗ୲୰ୣୱୱ ౪౨౩౩ ୗ୦ୣୟ୰୰ୟ୲ୣ ൌ ౪౨ ൌ

TAINSTRUMENTS.COM 6LPSOH6WHDG\6KHDU)ORZ

Top plate Area = A x(t) Velocity = V0 Force = F

y y Bottom Plate Velocity = 0 x F Shear Stress, Pascals σ = A

x(t) σ γ = η = Shear Strain, % Viscosity, Pa⋅s y γ

γ -1 γ = Shear Rate, sec t

TAINSTRUMENTS.COM 7RUVLRQ)ORZLQ3DUDOOHO3ODWHV

Ω r θ

h

Stress (σ) ߪൌ మ ൈM ഏయ r = plate radius h = distance between plates γ ߛൌ ൈθ M = torque (μN.m) Strain ( ) θ = Angular motor deflection (radians) Ω= Motor angular velocity (rad/s) Ω Strain rate (ߛሶ) ߛሶ ൌ ൈ

TAINSTRUMENTS.COM 7$,QVWUXPHQWV5KHRPHWHUV

TAINSTRUMENTS.COM 5RWDWLRQDO5KHRPHWHUVDW7$

ARES G2 DHR

Controlled Strain Controlled Stress Dual Head Single Head SMT CMT

TAINSTRUMENTS.COM 5RWDWLRQDO5KHRPHWHU'HVLJQV

Dual head or SMT Single head or CMT Separate motor & transducer Combined motor & transducer

Displacement Measured Transducer Sensor Torque (Stress) Measured Strain or Rotation Non-Contact Drag Cup Motor

Applied Torque Sample (Stress)

Applied Strain or Direct Drive ^ƚĂƚŝĐWůĂƚĞStatic Plate Rotation Motor

Note: With computer feedback, DHR and AR can work in controlled strain/shear rate, and ARES can work in controlled stress. TAINSTRUMENTS.COM :KDWGRHVD5KHRPHWHUGR"

Rheometer – an instrument that measures both viscosity and viscoelasticity of fluids, semi-solids and solids

It can provide information about the material’s: Viscosity - defined as a material’s resistance to deformation and is a function of shear rate or stress, with time and temperature dependence

Viscoelasticity – is a property of a material that exhibits both viscous and elastic character. Measurements of G’, G”, tan δ with respect to time, temperature, frequency and stress/strain are important for characterization.

A Rheometer works simply by relating a materials property from how hard it’s being pushed, to how far it moves

by commanding torque (stress) and measuring angular displacement (strain) by commanding angular displacement (strain) and measuring torque (stress)

TAINSTRUMENTS.COM +RZGR5KHRPHWHUVZRUN"

From the definition of rheology,

the science of flow and deformation of matter or the study of stress (Force / Area) – deformation (Strain or Strain rate) relationships.

Fundamentally a rotational rheometer will apply or measure: 1. Torque (Force) 2. Angular Displacement 3. Angular Velocity

TAINSTRUMENTS.COM 7RUTXHÆ 6KHDU6WUHVV

In a rheometer, the stress is calculated from the torque.

The formula for stress is: σ сΜ п <σ Where σ = Stress (Pa or Dyne/cm2) Μ = torque in N.mor gm.cm

<σ = Stress Constant

The stress constant, <σ, is a geometry dependent factor

TAINSTRUMENTS.COM $QJXODU'LVSODFHPHQWÆ 6KHDU6WUDLQ

In a SMT Rheometer, the angular displacement is directly applied by a motor.

The formula for strain is: γ с<γ п θ йγ сγ п ϭϬϬ where γ = Strain

<γ = Strain Constant θ = Angular motor deflection (radians)

The strain constant, <γ, is a geometry dependent factor

TAINSTRUMENTS.COM (TXDWLRQIRU0RGXOXV

Describe In Spec Correctly

σ M ⋅ Kσ G = γ = θ ⋅ Kγ

Geometric Rheological Constitutive Raw rheometer Shape Parameter Equation Specifications Constants

The equation of motion and other relationships have been used to determine the appropriate equations to convert machine parameters (torque, angular velocity, and angular displacement) to rheological parameters.

TAINSTRUMENTS.COM $QJXODU9HORFLW\Æ 6KHDU5DWH

In a SMT rheometer, the angular speed is directly controlled by the motor).

The formula for shear rate is:

ߛሶ ൌܭఊ ൈ: where ߛሶ = Shear rate <γ = Strain Constant Ω = Motor angular velocity in rad/sec

The strain constant, <γ, is a geometry dependent factor

TAINSTRUMENTS.COM (TXDWLRQIRU9LVFRVLW\

Describe In Spec Correctly σ ⋅ η = = M Kσ γ Ω ⋅ Kγ

Geometric Rheological Constitutive Raw rheometer Shape Parameter Equation Specifications Constants

The equation of motion and other relationships have been used to determine the appropriate equations to convert machine parameters (torque, angular velocity, and angular displacement) to rheological parameters.

TAINSTRUMENTS.COM 'LVFRYHU\+\EULG5KHRPHWHU6SHFLILFDWLRQV

Specification HR-3 HR-2 HR-1 Bearing Type, Thrust Magnetic Magnetic Magnetic Bearing Type, Radial Porous Carbon Porous Carbon Porous Carbon Motor Design Drag Cup Drag Cup Drag Cup Minimum Torque (nN.m) Oscillation 0.5 2 10 ,ZͲϮ ,ZͲϯ Minimum Torque (nN.m) Steady 51020 ,ZͲϭ Shear Maximum Torque (mN.m) 200 200 150 Torque Resolution (nN.m) 0.05 0.1 0.1 Minimum Frequency (Hz) 1.0E-07 1.0E-07 1.0E-07 Maximum Frequency (Hz) 100 100 100 Minimum Angular Velocity (rad/s) 0 0 0 Maximum Angular Velocity (rad/s) 300 300 300 Displacement Transducer Optical Optical Optical encoder encoder encoder Optical Encoder Dual Reader Standard N/A N/A Displacement Resolution (nrad) 2 10 10 Step Time, Strain (ms) 15 15 15 Step Time, Rate (ms) 5 5 5 DHR - DMA mode (optional) Normal/Axial Force Transducer FRT FRT FRT Maximum Normal Force (N) 50 50 50 Motor Control FRT Minimum Force (N) Oscillation 0.1 Normal Force Sensitivity (N) 0.005 0.005 0.01 Maximum Axial Force (N) 50 Minimum Displacement (μm) 1.0 Normal Force Resolution (mN) 0.5 0.5 1 Oscillation Maximum Displacement (μm) 100 Oscillation Displacement Resolution (nm) 10 Axial Frequency Range (Hz) 1 x 10-5 to 16

TAINSTRUMENTS.COM $5(6*5KHRPHWHU 6SHFLILFDWLRQV

Force/Torque Rebalance Transducer (Sample Stress) Transducer Type Force/Torque Rebalance Transducer Torque Motor Brushless DC Transducer Normal/Axial Motor Brushless DC Minimum Torque (μN.m) Oscillation 0.05 Minimum Torque (μN.m) Steady Shear 0.1 Maximum Torque (mN.m) 200 Torque Resolution (nN.m) 1 Transducer Normal/Axial Force Range (N) 0.001 to 20 Transducer Bearing Groove Compensated Air

Driver Motor (Sample Deformation) Maximum Motor Torque (mN.m) 800 Orthogonal Superposition (OSP) and Motor Design Brushless DC DMA modes Motor Bearing Jeweled Air, Sapphire Motor Control FRT Displacement Control/ Sensing Optical Encoder Strain Resolution (μrad) 0.04 Minimum Transducer Force (N) 0.001 Oscillation Minimum Angular Displacement (μrad) 1 Maximum Transducer Force 20 Oscillation (N) Maximum Angular Displacement (μrad) Unlimited Minimum Displacement (μm) 0.5 Steady Shear Oscillation -6 Angular Velocity Range (rad/s) 1x 10 to 300 Maximum Displacement (μm) 50 Angular Frequency Range (rad/s) 1x 10-7 to 628 Oscillation Step Change, Velocity (ms) 5 Displacement Resolution (nm) 10 Step Change, Strain (ms) 10 Axial Frequency Range (Hz) 1 x 10-5 to 16

TAINSTRUMENTS.COM *HRPHWU\2SWLRQV

Concentric Cone and Parallel Torsion Cylinders Plate Plate Rectangular

Very Low Very Low Very Low Solids to Medium to High Viscosity Viscosity Viscosity to Soft Solids Water to Steel

TAINSTRUMENTS.COM &KRRVLQJD*HRPHWU\6L]H

Assess the ‘viscosity’ of your sample When a variety of cones and plates are available, select diameter appropriate for viscosity of sample Low viscosity (milk) - 60mm geometry Medium viscosity (honey) - 40mm geometry High viscosity (caramel) – 20 or 25mm geometry Examine data in terms of absolute instrument variables torque/displacement/speed and modify geometry choice to move into optimum working range You may need to reconsider your selection after the first run!

TAINSTRUMENTS.COM 3DUDOOHO3ODWH

Strain Constant: ܭఊ ൌ (to convert angular velocity, rad/sec, to shear rate, 1/sec, at the edge or angular displacement, radians, to shear strain (unitless) at the edge. The radius, r, and the gap, h, are expressed in meters)

'ĂƉ;ŚͿ Stress Constant: ܭ ൌ ଶ ఙ గయ (to convert torque, N⋅m, to shear stress at the ŝĂŵĞƚĞƌ;Ϯ⋅⋅⋅ƌͿ edge, Pa, for Newtonian fluids. The radius, r, is expressed in meters)

TAINSTRUMENTS.COM :KHQWRXVH3DUDOOHO3ODWHV

Low/Medium/High Viscosity Samples with long relaxation time Liquids Temperature Ramps/ Sweeps Soft Solids/Gels Materials that may slip Thermosetting materials Crosshatched or Sandblasted plates Samples with large particles Small sample volume

TAINSTRUMENTS.COM 3ODWH'LDPHWHUV

Shear Stress

20 mm

40 mm

60 mm

ʹ As diameter decreases, shear stress increases ߪൌܯ ߨݎଶ

TAINSTRUMENTS.COM 3ODWH*DSV

Shear Rate 2 mm Increases

1 mm

0.5 mm

ݎ As gap height decreases, shear rate increases ߛሶ ൌȳ ݄

TAINSTRUMENTS.COM (IIHFWLYH6KHDU5DWHYDULHVDFURVVD3DUDOOHO3ODWH

For a given angle of deformation, there is a greater arc of deformation at the edge of the plate than at the center

,ݔ dx increases further from the center݀ ߛൌ ݄ h stays constant

TAINSTRUMENTS.COM 6KHDU5DWHLV1RUPDOL]HGDFURVVD&RQH

The cone shape produces a smaller gap height closer to inside, so the shear on the sample is constant

ݔ݀ ߛൌ h increases proportionally to dx, γ is uniform ݄

TAINSTRUMENTS.COM &RQHDQG3ODWH

ଵ Strain Constant: ܭఊ ൌఉ (to convert angular velocity, rad/sec, to shear rate. 1/sec, or angular displacement, radians, to shear strain, which is unit less. The angle, β, is expressed in radians)

ܭ ൌ ଷ Stress Constant: ఙ ଶగయ

(to convert torque, N⋅m, to shear stress, Pa. The radius, r, is expressed in meters)

Diameter (2⋅⋅⋅r) Truncation (gap)

TAINSTRUMENTS.COM :KHQWRXVH&RQHDQG3ODWH

Very Low to High Viscosity Liquids High Shear Rate measurements Normal Stress Growth Unfilled Samples Isothermal Tests Small Sample Volume

TAINSTRUMENTS.COM &RQH'LDPHWHUV

Shear Stress

20 mm

40 mm

60 mm

͵ As diameter decreases, shear stress increases ߪൌܯ ʹߨݎଷ

TAINSTRUMENTS.COM &RQH$QJOHV

Shear Rate Increases

2 °

1 °

0.5 °

ͳ As cone angle decreases, shear rate increases ߛሶ ൌȳ ߚ

TAINSTRUMENTS.COM /LPLWDWLRQVRI&RQHDQG3ODWH

Typical Truncation Heights: 1° degree ~ 20 - 30 microns 2° degrees ~ 60 microns 4° degrees ~ 120 microns

Cone & Plate Truncation Height = Gap

Gap must be > or = 10 [particle size]!!

TAINSTRUMENTS.COM &RUUHFW6DPSOH/RDGLQJ

× Under Filled sample: Lower torque contribution

× Over Filled sample: Additional stress from drag along the edges

9 Correct Filling

TAINSTRUMENTS.COM &RQFHQWULF&\OLQGHU

ݎ ଶ ݎ ଶ Strain Constant: ͳ ʹ ܭఊ ൌ ଶ ଶ ݎʹ ݎͳ (to convert angular velocity, rad/sec, to shear rate, 1/sec, or angular displacement, radians, to shear

strain (unit less). The radii, r1 (inner) and r2 (outer), are expressed in meters)

* ݎ ଶ ݎ ଶ Stress Constant: ଵ ͳ ʹ ܭఙ ൌସగ ଶ ଶ ݎʹ ݎͳ

(to convert torque, N⋅m, to shear stress, Pa. The bob length, l, and the radius, r, are expressed in meters)

*Note including end correction factor. See TRIOS Help TAINSTRUMENTS.COM 'RXEOH:DOO

Use for very low viscosity systems (<1 mPas)

r1

r2 h r3

r4

ଶ ଶ ݎͳ ݎʹ Strain Constant: ܭఊ ൌ ଶ ଶ ݎʹ െݎͳ మ మ ଵ ାଶ Stress Constant: ܭఙ ൌ మ మ మ ସగήଶ ଵ ାଷ ARES Gap Settings: standard operating gap DW = 3.4 mm narrow operating gap DW = 2.0 mm

Use equation Gap > 3 × (R2 –R1) TAINSTRUMENTS.COM :KHQWR8VH&RQFHQWULF&\OLQGHUV

Low to Medium Viscosity Liquids Unstable Dispersions and Slurries Minimize Effects of Evaporation Weakly Structured Samples (Vane) High Shear Rates

TAINSTRUMENTS.COM 3HOWLHU &RQFHQWULF&\OLQGHUV

TAINSTRUMENTS.COM 7RUVLRQ5HFWDQJXODU

ݐ ܭ ൌ ఊ ௧ ଶ ݈ ͳ െ ͲǤ͵ͺ ௪ w = Width l = Length ͵ଵǤ଼ t = Thickness ܭ ൌ ௪ ఛ ݓήݐଶ

Advantages: Disadvantages:

High modulus samples No pure Torsion mode for Small temperature high strains gradient Simple to prepare

Torsion cylindrical also available

TAINSTRUMENTS.COM 7RUVLRQDQG'0$0HDVXUHPHQWV

Torsion and DMA geometries allow solid samples to be characterized in a temperature controlled environment

Torsion measures G’, G”, and Tan δ DMA measures E’, E”, and Tan δ ARES G2 DMA is standard function (50 μm amplitude) DMA is an optional DHR function (100 μm amplitude)

Rectangular and DMA 3-point bending and tension cylindrical torsion (cantilever not shown)

TAINSTRUMENTS.COM *HRPHWU\2YHUYLHZ

Geometry Application Advantage Disadvantage

Cone/plate fluids, melts true viscosities temperature ramp difficult viscosity > 10mPas

Parallel Plate fluids, melts easy handling, shear gradient across viscosity > 10mPas temperature ramp sample

Couette low viscosity samples high shear rate large sample volume < 10 mPas

Double Wall Couette very low viscosity high shear rate cleaning difficult samples < 1mPas

Torsion Rectangular solid polymers, glassy to rubbery Limited by sample stiffness composites state

Limited by sample stiffness Solid polymers, films, Glassy to rubbery DMA (Oscillation and Composites state stress/strain)

TAINSTRUMENTS.COM 5KHRPHWHU&DOLEUDWLRQVDQG 3HUIRUPDQFH9HULILFDWLRQ

TAINSTRUMENTS.COM '+5² &DOLEUDWLRQ2SWLRQV

Instrument Calibrations

Inertia (Service)

Rotational Mapping

Geometry Calibrations:

Inertia

Friction

Gap Temperature Compensation

Rotational Mapping

Details in Appendix #4

TAINSTRUMENTS.COM $5(6*² &DOLEUDWLRQ2SWLRQV

Instrument Calibrations Transducer Temperature Offsets Phase Angle (Service) Measure Gap Temperature Compensation

Geometry Calibrations: Compliance and Inertia (from table) Gap Temperature Compensation

Details in Appendix #4

TAINSTRUMENTS.COM 9HULI\5KHRPHWHU3HUIRUPDQFH

Rheometers are calibrated from the factory and again at installation. TA recommends routine validation or confidence checks using standard oils or Polydimethylsiloxane (PDMS).

PDMS is verified using a 25 mm parallel plate. Oscillation - Frequency Sweep: 1 to 100 rad/s with 5% strain at 30°C Verify modulus and frequency values at crossover

Standard silicone oils can be verified using cone, plate or concentric cylinder configurations. Flow – Ramp: 0 to 88 Pa at 25°C using a 60 mm 2° cone

Service performs this test at installation

TAINSTRUMENTS.COM 3'06)UHTXHQF\6ZHHS5HVXOWV

TAINSTRUMENTS.COM /RDG6WDQGDUG2LO

Set Peltier temperature to 25°C and equilibrate. Zero the geometry gap

Load sample Be careful not to introduce air bubbles!

Set the gap to the trim gap

Lock the head and trim with non-absorbent tool Important to allow time for temperature equilibration.

Go to geometry gap and initiate the experiment.

TAINSTRUMENTS.COM )ORZ5DPS² 6WDQGDUG2LO 6HUYLFH7HVW

TAINSTRUMENTS.COM 6HWWLQJXS5KHRORJLFDO([SHULPHQWV )ORZ7HVWV

TAINSTRUMENTS.COM 9LVFRVLW\'HILQLWLRQ

Viscosity is… “lack of slipperiness” synonymous with internal friction resistance to flow

The Units of Viscosity are … SI unit is the Pascal.second (Pa.s) cgs unit is the Poise 10 Poise = 1 Pa.s 1 cP (centipoise) = 1 mPa.s (millipascal second)

TAINSTRUMENTS.COM (TXDWLRQIRU9LVFRVLW\

Describe In Spec Correctly σ ⋅ η = = M Kσ γ Ω ⋅ Kγ

Geometric Rheological Constitutive Raw rheometer Shape Parameter Equation Specifications Constants

TAINSTRUMENTS.COM 7\SLFDO9LVFRVLW\9DOXHV 3DV

6 Asphalt Binder ------100,000 6 Polymer Melt ------1,000 6 Molasses ------100 6 Liquid Honey ------10 Need for 6 Glycerol ------1 Log scale 6 Olive Oil ------0.01 6 Water ------0.001 6 Air ------0.00001

TAINSTRUMENTS.COM 1HZWRQLDQDQG1RQ1HZWRQLDQ)OXLGV

Newtonian Fluids - constant proportionality between shear stress and shear-rate

Non-Newtonian Fluids - Viscosity is time or shear rate dependent Time:

At constant shear-rate, if viscosity

Decreases with time – Thixotropy

Increases with time - Rheopexy Shear-rate:

Shear - thinning

Shear - thickening

TAINSTRUMENTS.COM &KDUDFWHULVWLF'LDJUDPVIRU1HZWRQLDQ)OXLGV

Ideal Yield Stress (Bingham Yield) Pa.s , Pa η, σ

γ ,1/s or σ, Pa γ ,1/s

TAINSTRUMENTS.COM &KDUDFWHULVWLF'LDJUDPVIRU6KHDU7KLQQLQJ)OXLGV

105 105

103 103 Pa.s 101 Pa.s 101 η, η, 10-1 10-1 10-6 10-4 10-2 100 102 104 10-1 10-0 10-1 102 103 ,1/s σ, Pa

105 ,GHDO

σ 101

10-1 10-6 10-4 10-2 100 102 104 γ ,1/s

TAINSTRUMENTS.COM &KDUDFWHULVWLF'LDJUDPVIRU6KHDU7KLFNHQLQJ)OXLGV

Dilatant material resists deformation more than in proportion to the applied

Pa.s force (shear-thickening) η, Cornstarch in water or sand Log on the beach are actually dilatant fluids, since they do not show the time- dependent, shear-induced change required in order to Log ߛሶ,1/s be labeled rheopectic

TAINSTRUMENTS.COM 1RQ1HZWRQLDQ7LPH'HSHQGHQW)OXLGV

Rheopectic materials become more viscous Rheopectic with increasing time of applied force Higher concentration latex dispersions and Shear Rate = Constant plastisol paste materials exhibit rheopectic Viscosity behavior Thixotropic Thixotropic materials become more fluid with increasing time of applied time force Coatings and inks can display thixotropy when sheared due to structure breakdown

TAINSTRUMENTS.COM )ORZ([SHULPHQWV

Flow Experiments Constant shear rate/stress (or Peak hold) Continuous stress/rate ramp and down Stepped flow (or Flow sweep) Steady state flow Flow temperature ramp

TAINSTRUMENTS.COM &RQVWDQW6KHDU5DWH6WUHVV

Constant rate vs. time

Constant stress vs. time Stress /Rate

USES Single point testing Scope the time for steady state under certain rate

TAINSTRUMENTS.COM &RQVWDQW6KHDU5DWH6WUHVV

3.500 4.000 Hand Wash Rate 1/s

3.500 3.000

3.000 2.500

2.500 viscosity (Pa.s) viscosity 2.000

2.000

1.500 shear stress (Pa) Viscosity at 1 1/s is 2.8 Pa⋅s 1.500

1.000 1.000

0.5000 0.5000

0 0 0 5.0000 10.000 15.000 20.000 25.000 30.000 time (s)

TAINSTRUMENTS.COM &RQWLQXRXV5DPS

Deformation Stress is applied to material at a constant m =Stress rate rate. Resultant strain (Pa/min) is monitored with time.

time (min)

USES Yield stress Scouting Viscosity Run

TAINSTRUMENTS.COM 6WUHVV5DPS)ORZ0HGLD'LVSHUVLRQ

TAINSTRUMENTS.COM 7KL[RWURSLF/RRS &RQWLQXRXV5DPS8SDQG'RZQ

Deformation Stress is first increased, σ then decreased, at a constant rate. Resultant strain is monitored with time. time

USES “Pseudo-thixotropy” from Hysteresis loop

TAINSTRUMENTS.COM 8S 'RZQ)ORZ&XUYHV 5HSHDWV

Run in Stress Control TA Instruments 500.0

400.0

300.0 ZĞĚ͗&ŝƌƐƚĐǇĐůĞ ůƵĞ͗^ĞĐŽŶĚĐǇĐůĞ 200.0

shear stress (Pa) FORDB3.04F-Up step FORDB3.04F-Down step FORDB3.05F-Up step 100.0 FORDB3.05F-Down step

0 0 0.1000 0.2000 0.3000 0.4000 0.5000 shear rate (1/s)

TAINSTRUMENTS.COM 6WHSSHGRU6WHDG\6WDWH)ORZ

Deformation σ Data point saved Stress is applied to sample. Žƌ Viscosity measurement is taken ߛሶ when material has reached steady state flow. The stress is increased(logarithmically) and the time process is repeated yielding a viscosity flow curve.

Delay time σ USES Žƌ Steady State Flow ߛሶ Viscosity Flow Curves γ or σ = Constant Yield Stress Measurements

time

TAINSTRUMENTS.COM 6WHSSHGRU6WHDG\6WDWH)ORZ

A series of logarithmic stress steps allowed to reach steady state, each one giving a single viscosity data point:

Data at each Shear Rate

Shear Thinning Region

Time Viscosity

η = σ / γ/ Shear Rate, 1/s (d dt)

TAINSTRUMENTS.COM '+5DQG$5(6*6WHDG\6WDWH)ORZ

Control variables: Shear rate Velocity Torque Shear stress

Steady state algorithm

TAINSTRUMENTS.COM )ORZ6ZHHSV :DWHU%DVHG3DLQWZLWK6ROYHQW7UDS

TAINSTRUMENTS.COM &RPSDULVRQRI&RXJK6\UXSV

0.8000 ^ĂŵƉůĞϭͲ&ůŽǁƐƚĞƉ ^ĂŵƉůĞϮͲ&ůŽǁƐƚĞƉ 0.7000 Which material would do a better job 0.6000 coating your throat?

0.5000

0.4000 viscosity (Pa.s) viscosity 0.3000

0.2000

0.1000

0 0.1000 1.000 10.00 100.0 1000 shear rate (1/s)

TAINSTRUMENTS.COM &RPSDULVRQRI7ZR/DWH[3DLQWV

10000 A.01F-Flow step Low shear rates B>A B.01F-Flow step

1000

100.0

viscosity (Pa.s) 10.00 Medium shear rates A>B

1.000

High shear rates B>A

0.1000 1.000E-4 1.000E-3 0.01000 0.1000 1.000 10.00 100.0 1000 shear rate (1/s)

TAINSTRUMENTS.COM )ORZ7HPSHUDWXUH5DPS

Hold the rate or stress yyyy constant whilst ramping the temperature.

time (min)

USES Measure the viscosity change vs. temperature

TAINSTRUMENTS.COM 9LVFRVLW\7HPSHUDWXUH'HSHQGHQFH

Notice a nearly 2 decade decrease in viscosity. This displays the importance of thermal equilibration of the sample prior to testing. i.e. Conditioning Step or equilibration time for 3 to 5 min

TAINSTRUMENTS.COM )ORZ7HVWLQJ&RQVLGHUDWLRQV

Small gaps give high shear rates Be careful with small gaps:

Gap errors (gap temperature compensation) and shear heating can cause large errors in data.

Recommended gap is between 0.5 to 2.0 mm.

Secondary flows can cause increase in viscosity curve Be careful with data interpretation at low shear rates Surface tension can affect measured viscosity, especially with aqueous materials

TAINSTRUMENTS.COM :DWHUDW&² 6HFRQGDU\)ORZ

Surface tension at low torques

Secondary flows at high shear rates

TAINSTRUMENTS.COM :DOO6OLS

Wall slip can manifest as “apparent double yielding” Can be tested by running the same test at different gaps For samples that don’t slip, the results will be independent of the gap

TAINSTRUMENTS.COM 6KHDU7KLQQLQJRU6DPSOH,QVWDELOLW\"

When Stress Decreases with Shear Rate, it indicates that sample is leaving the gap

TAINSTRUMENTS.COM )ORZ7HVWLQJ&RQVLGHUDWLRQV

Edge Failure – Sample leaves gap because of normal forces Look at stress vs. shear rate curve – stress should not decrease with increasing shear rate – this indicates sample is leaving gap Possible Solutions: use a smaller gap or smaller angle so that you get the same shear rate at a lower angular velocity if appropriate (i.e. Polymer melts) make use of Cox Merz Rule η γ η* () ≡ ω ( )

TAINSTRUMENTS.COM 9LVFRHODVWLFLW\

TAINSTRUMENTS.COM (ODVWLF%HKDYLRURIDQ,GHDO6ROLG

Hooke’s Law of Elasticity: Stress = Modulus ⋅ Strain

γ γ γ 1 2 3

3

2

^ƚƌĞƐƐ;ʍͿ 1

1 2 3 ^ƚƌĂŝŶ;࠹Ϳ

TAINSTRUMENTS.COM (ODVWLF%HKDYLRURIDQ,GHDO6ROLG

Hooke’s Law of Elasticity: Stress = Modulus ⋅ Strain E > E >E

ߪ ܧൌ γ γ γ ߛ 1 2 3

TAINSTRUMENTS.COM 9LVFRXV%HKDYLRURIDQ,GHDO/LTXLG

Newton’s Law: stress = coefficient of viscosity ⋅ shear rate Ș ߪൌKήߛሶ ^ƚƌĞƐƐ;ʍͿ

^ŚĞĂƌZĂƚĞ;࠹Ϳ

TAINSTRUMENTS.COM 9LVFRXV%HKDYLRURIDQ,GHDO/LTXLG ߪ Newton’s Law: stress= coefficient of viscosity ⋅ shear rate Ʉൌ ߛሶ Ș < Ș < Ș

TAINSTRUMENTS.COM sŝƐĐŽĞůĂƐƚŝĐĞŚĂǀŝŽƌ ʍ сΎɸ нɻΎĚɸͬĚƚ

<ĞůǀŝŶͲsŽŝŐƚDŽĚĞů;ƌĞĞƉͿ DĂǆǁĞůůDŽĚĞů;^ƚƌĞƐƐZĞůĂǆĂƚŝŽŶͿ

L1

L2

sŝƐĐŽĞůĂƐƚŝĐDĂƚĞƌŝĂůƐ͗&ŽƌĐĞ ĚĞƉĞŶĚƐŽŶďŽƚŚĞĨŽƌŵĂƚŝŽŶĂŶĚ ZĂƚĞŽĨĞĨŽƌŵĂƚŝŽŶĂŶĚǀŝĐĞǀĞƌƐĂ͘ 9LVFRHODVWLFLW\'HILQHG

Range of Material Behavior Liquid Like------Solid Like Ideal Fluid ----- Most Materials -----Ideal Solid Purely Viscous ----- Viscoelastic ----- Purely Elastic

Viscoelasticity: Having both viscous and elastic properties

Materials behave in the linear manner, as described by Hooke and Newton, only on a small scale in stress or deformation.

TAINSTRUMENTS.COM 3LWFK'URS([SHULPHQW

Long deformation time: pitch behaves like a highly viscous liquid th 9 drop fell July 2013 Short deformation time: pitch behaves like a solid

Started in 1927 by Thomas Parnell in Queensland, Australia ŚƚƚƉ͗ͬͬǁǁǁ͘ƚŚĞĂƚůĂŶƚŝĐ͘ĐŽŵͬƚĞĐŚŶŽůŽŐǇͬĂƌĐŚŝǀĞͬϮϬϭϯͬϬϳͬƚŚĞͲϯͲŵŽƐƚͲĞǆĐŝƚŝŶŐͲǁŽƌĚƐͲŝŶͲƐĐŝĞŶĐĞͲƌŝŐŚƚͲŶŽǁͲƚŚĞͲƉŝƚĐŚͲĚƌŽƉƉĞĚͬϮϳϳϵϭϵͬ

TAINSTRUMENTS.COM 7LPH'HSHQGHQW9LVFRHODVWLF%HKDYLRU

T is short [< 1s] T is long [24 hours]

TAINSTRUMENTS.COM 7LPH'HSHQGHQW9LVFRHODVWLF%HKDYLRU

Silly Putties have different characteristic relaxation times Dynamic (oscillatory) testing can measure time-dependent viscoelastic properties more efficiently by varying frequency (deformation time)

TAINSTRUMENTS.COM 9LVFRHODVWLFLW\'HERUDK1XPEHU

Old Testament Prophetess who said (Judges 5:5): "The Mountains ‘Flowed’ before the Lord"

Everything Flows if you wait long enough!

Deborah Number, De - The ratio of a characteristic relaxation time of a material (τ) to a characteristic time of the relevant deformation process (T).

Ğсτͬd

TAINSTRUMENTS.COM 'HERUDK1XPEHU

Hookean elastic solid - Ĳ is infinite Newtonian Viscous Liquid - Ĳ is zero Polymer melts processing - Ĳ may be a few seconds

High De Solid-like behavior Low De Liquid-like behavior

IMPLICATION: Material can appear solid-like because 1) it has a very long characteristic relaxation time or 2) the relevant deformation process is very fast

TAINSTRUMENTS.COM 7LPHDQG7HPSHUDWXUH 5HODWLRQVKLS

(E' or G') (E' or G') (E" or G") (E" or G")

log Frequency Temperature

log Time log Time

TAINSTRUMENTS.COM /LQHDU9LVFRHODVWLFLW\5HJLRQ /95 'HILQHG

"If the deformation is small, or applied sufficiently slowly, the molecular arrangements are never far from equilibrium.

The mechanical response is then just a reflection of dynamic processes at the molecular level which go on constantly, even for a system at equilibrium.

This is the domain of LINEAR VISCOELASTICITY.

The magnitudes of stress and strain are related linearly, and the behavior for any liquid is completely described by a single function of time."

Mark, J., et. al., Physical Properties of Polymers, American Chemical Society, 1984, p. 102.

TAINSTRUMENTS.COM ,PSRUWDQFHRI/95

͛;Žƌ'͛Ϳ͕͟;Žƌ'͟Ϳ͕ƚĂŶδ͕ηΎ

Measuring linear viscoelastic properties helps us bridge the gap between molecular structure and product performance

TAINSTRUMENTS.COM 6HWWLQJXS5KHRORJLFDO([SHULPHQWV 2VFLOODWRU\7HVWV

TAINSTRUMENTS.COM 8QGHUVWDQGLQJ2VFLOODWLRQ([SHULPHQWV

Define Oscillation Testing

Approach to Oscillation Experimentation Stress and Strain Sweep Time Sweep Frequency Sweep Temperature Ramp Temperature Sweep (TTS)

TAINSTRUMENTS.COM :KDWLV2VFLOODWLRQ"

Phase angle δ Strain, ε

Stress, σΎ

Dynamic stress applied sinusoidally User-defined Stress or Strain amplitude and frequency

TAINSTRUMENTS.COM )UHTXHQF\'HILQHG

Time to complete one oscillation Frequency is the inverse of time Units Angular Frequency = radians/second Frequency = cycles/second (Hz) Rheologist must think in terms of rad/s. 1 Hz = 6.28 rad/s

TAINSTRUMENTS.COM )UHTXHQF\

ω = 6.28 rad/s

ω = 12.560rad/s

0 0 0 0

dŝŵĞсϭƐĞĐ ω = 50 rad/s

TAINSTRUMENTS.COM $PSOLWXGH6WUDLQRU6WUHVV

Strain and stress are calculated from peak amplitude in the displacement and torque waves, respectively.

0 0 0 0

dŝŵĞсϭƐĞĐ

TAINSTRUMENTS.COM '\QDPLF0HFKDQLFDO7HVWLQJ

Deformation An oscillatory (sinusoidal) deformation (stress or strain) is applied to a sample. Response The material response (strain or stress) is measured.

The phase angle δ, or phase shift, between the deformation Phase angle δ and response is measured.

TAINSTRUMENTS.COM '\QDPLF7HVWLQJ5HVSRQVHIRU&ODVVLFDO([WUHPHV

Purely Elastic Response Purely Viscous Response (Hookean Solid) (Newtonian Liquid) δ сϬ° δ сϵϬ°

Strain Strain

Stress Stress

TAINSTRUMENTS.COM '\QDPLF7HVWLQJ9LVFRHODVWLF0DWHULDO5HVSRQVH

Phase angle 0°< δ < 90°

Strain

Stress

TAINSTRUMENTS.COM 9LVFRHODVWLF3DUDPHWHUV&RPSOH[(ODVWLF 9LVFRXV6WUHVV

The stress in a dynamic experiment is referred to as the complex stress σ* The complex stress can be separated into two components: 1) An elastic stress in phase with the strain. σ' = σ*cosδ σ' is the degree to which material behaves like an elastic solid. 2) A viscous stress in phase with the strain rate. σ" = σ*sinδ σ" is the degree to which material behaves like an ideal liquid.

Phase angle δ Complex Stress, σ* σ* = σ' + iσ"

Complex number: ݔ݅ݕ ൌ ݔଶ ݕଶ The material functions can be described in Strain, ε terms of complex variables having both real and imaginary parts. Thus, using the relationship:

TAINSTRUMENTS.COM 9LVFRHODVWLF3DUDPHWHUV

כୗ୲୰ୣୱୱ כ The Modulus: Measure of materials overall resistance to ൌ ୗ୲୰ୟ୧୬ deformation. The Elastic (Storage) Modulus: כୗ୲୰ୣୱୱ Measure of elasticity of material. ᇱ ൌ Ɂ The ability of the material to store ୗ୲୰ୟ୧୬ energy. The Viscous (loss) Modulus: כ The ability of the material to ̶ ൌ ୗ୲୰ୣୱୱ Ɂ dissipate energy. Energy lost as ୗ୲୰ୟ୧୬ heat.

Tan Delta: ̶ Measure of material damping - ୋ Ɂ ൌ ᇱ such as vibration or sound ୋ damping.

TAINSTRUMENTS.COM 6WRUDJHDQG/RVVRID9LVFRHODVWLF0DWHULDO

RUBBER BALL y LOSS (G”) TENNIS BALL y

STORAGE (G’)

G* Dynamic measurement G" represented as a vector Phase angle δ G'

TAINSTRUMENTS.COM &RPSOH[9LVFRVLW\

The viscosity measured in an oscillatory experiment is a Complex Viscosity much the way the modulus can be expressed as the complex modulus. The complex viscosity contains an elastic component and a term similar to the steady state viscosity.

The Complex viscosity is defined as: Ș* = Ș’ + i Ș” or Ș* = G*/Ȧ

Note: frequency must be in rad/sec!

TAINSTRUMENTS.COM '\QDPLF5KHRORJLFDO3DUDPHWHUV

Parameter Shear Elongation Units

Strain ɶсɶϬƐŝŶ;ʘƚͿ ɸ сɸϬ ƐŝŶ;ʘƚͿ ---

σ σ τ τ Stress с ϬƐŝŶ;ʘƚнɷͿ с ϬƐŝŶ;ʘƚнɷͿ Pa

Storage Modulus '͛с;σ ͬɶ ͿĐŽƐɷ ͛с;τ ͬɸ ͿĐŽƐɷ Pa (Elasticity) Ϭ Ϭ Ϭ Ϭ

Loss Modulus '͟с;σ ͬɶ ͿƐŝŶɷ ͟с;τ ͬɸ ͿƐŝŶɷ Pa (Viscous Nature) Ϭ Ϭ Ϭ Ϭ

Tan į 'ͬ͟'͛ ͬ͛͟ ---

Complex Modulus 'Ύ с;'͛Ϯн'͟ϮͿϬ͘ϱ Ύ с;͛Ϯн͟ϮͿϬ͘ϱ Pa

ηΎ η Ύ Ύ Complex Viscosity с'Ύͬʘ с ͬʘ Pa·sec

Cox-Merz Rule for Linear Polymers: η*(Ȧ) = η(ߛሶ) @ ߛሶ = Ȧ

TAINSTRUMENTS.COM 8QGHUVWDQGLQJ2VFLOODWLRQ([SHULPHQWV

Define Oscillation Testing

Approach to Oscillation Experimentation 1. Stress and Strain Sweep 2. Time Sweep 3. Frequency Sweep 4. Temperature Ramp 5. Temperature Sweep (TTS)

TAINSTRUMENTS.COM '\QDPLF6WUDLQRU6WUHVV6ZHHS

The material response to increasing deformation amplitude (strain or stress) is monitored at a constant frequency and Stress or strain Time temperature.

Main use is to determine LVR All subsequent tests require an amplitude found in the LVR Tests assumes sample is stable If not stable use Time Sweep to determine stability

TAINSTRUMENTS.COM '\QDPLF6WUDLQ6ZHHS0DWHULDO5HVSRQVH

Linear Region: Modulus Non-linear Region: independent Modulus is a function of strain of strain

G'

Stress

Constant γ сCritical Strain Slope Đ

Strain (amplitude)

TAINSTRUMENTS.COM 7HPSHUDWXUH'HSHQGHQFHRI/95

In general, the LVR is shortest when the sample is in its most solid form.

Solid G’

Liquid

% strain

TAINSTRUMENTS.COM )UHTXHQF\'HSHQGHQFHRI/95

LVR decreases with increasing frequency Modulus increases with increasing frequency

TAINSTRUMENTS.COM 6$26YHUVXV/$26:DYHIRUPV

Linear response to a sinusoidal excitation is sinusoidal and represented by the fundamental in the frequency domain

Nonlinear response to a sinusoidal excitation is not sinusoidal and represented in the frequency domain by the fundamental and the harmonics

TAINSTRUMENTS.COM /$26$QDO\VLVRI+LJKHU+DUPRQLFV

^K^ γ γ ω (t) = 0 sin( t) τ τ ω δ (t) = 0 sin( t+ )

γ γ ω >K^ (t) = 0 sin( t)

Fourier Series expansion: τ τ ω ϕ τ ω ϕ (t) = 1 sin( 1t+ 1) + 3 sin(3 1t+ 3) + τ ω ϕ 5 sin(5 1t+ 5) + ... τ ω ϕ = Σ n sin(n 1+ n) n=1 odd Lissajous plot: Stress vs. Strain (shown) or stress vs. Shear rate

TAINSTRUMENTS.COM '\QDPLF7LPH6ZHHS

The material response is monitored at a constant frequency, amplitude and

Stress or strain temperature. Time

USES Time dependent Thixotropy Cure Studies Stability against thermal degradation Solvent evaporation/drying

TAINSTRUMENTS.COM ,PSRUWDQFHRI7LPH6ZHHS

Important, but often overlooked Visually observe the sample Determines if properties are changing over the time of testing Complex Fluids or Dispersions

Preshear or effects of loading

Drying or volatilization (use solvent trap)

Thixotropic or Rheopectic Polymers

Degradation (inert purge)

Crosslinking

TAINSTRUMENTS.COM 7LPH6ZHHSRQ3((.0HOW 7KHUPDO6WDELOLW\

Under N2 Under air

TAINSTRUMENTS.COM 7LPH6ZHHSRQ/DWH[

ϭϬϬ͘Ϭ Structural Recovery after Preshear

ϴϬ͘ϬϬ

ϲϬ͘ϬϬ

G' (Pa) ϰϬ͘ϬϬ

ϮϬ͘ϬϬ

Ϭ 0 Ϯϱ͘ϬϬ ϱϬ͘ϬϬ ϳϱ͘ϬϬ ϭϬϬ͘Ϭ ϭϮϱ͘Ϭ ϭϱϬ͘Ϭ ϭϳϱ͘Ϭ ϮϬϬ͘Ϭ ϮϮϱ͘Ϭ time (s)

TAINSTRUMENTS.COM ,PSRUWDQFHRI:DLWLQJIRU6WUXFWXUH5HEXLOG

Sample “A” time sweep Delay after pre-shear = 150 sec Delay after pre-shear = 0 sec 100.0 100.0 G' (Pa) Pre-shear conditions: 100 1/s for 30 seconds

10.00 10.00 0 25.00 50.00 75.00 100.0 125.0 150.0 175.0 0.1000 1.000 10.00 100.0

time (s) osc. stress (Pa)

End of LVR is indicative of “Yield” or “Strength of Structure” Useful for Stability predictions (stability as defined by yield)

TAINSTRUMENTS.COM 6ROYHQW7UDS6\VWHPIRU(IIHFWLYH(YDSRUDWLRQ&RQWURO

Solvent trap cover picks up heat from Peltier Plate to insure uniform temperature

^ŽůǀĞŶƚŝŶ ^ŽůǀĞŶƚdƌĂƉŽǀĞƌ tĞůů

WĞůƚŝĞƌ WůĂƚĞ ^ĂŵƉůĞ

TAINSTRUMENTS.COM &XUHRID0LQXWH(SR[\

TA Instruments 1000000 G' 1000000 5 min 100000 100000

10000 G" 10000 G'' (Pa) 1000 Gel Point: G' = G" 1000 G' (Pa) t = 330 s 100.0 100.0

10.00 10.00

1.000 1.000 0 200.0 400.0 600.0 800.0 1000 1200 time (s)

TAINSTRUMENTS.COM )UHTXHQF\6ZHHS

The material response to increasing frequency (rate of deformation) is monitored at a constant amplitude (strain

ŵƉůŝƚƵĚĞ or stress) and temperature.

dŝŵĞ

Strain should be in LVR Sample should be stable Remember – Frequency is 1/time so low frequencies will take a long time to collect data – i.e. 0.001Hz is 1000 sec (over 16 min)

TAINSTRUMENTS.COM )UHTXHQF\6ZHHS0DWHULDO5HVSRQVH

Transition Rubbery Region Terminal Plateau Region Region

Glassy Region

1 2 Storage Modulus (E' or G') >ŽƐƐDŽĚƵůƵƐ;ΗŽƌ'ΗͿ

log Frequency (rad/s or Hz)

TAINSTRUMENTS.COM )UHTXHQF\6ZHHS 7LPH'HSHQGHQW9LVFRHODVWLF3URSHUWLHV

Frequency of modulus crossover correlates with Relaxation Time

TAINSTRUMENTS.COM &R[0HU] ([DPSOH /'3(DW&

η γ η* () ≡ ω ( )

Flow instability Z

W

LDPE Freq sweep 2mm gap – Cox Merz LDPE shear rate 1mm gap LDPE Shear rate 2 mm gap

TAINSTRUMENTS.COM ,PSRUWDQFHRI)UHTXHQF\6ZHHSV

High and low rate (short and long time) properties Viscosity Information - Zero Shear Viscosity, shear thinning Elasticity (reversible deformation) in materials MW & MWD differences polymer melts and solutions Finding yield in gelled dispersions Can extend time or frequency range with TTS

3.4 G' § M · η ≈ M 3.4 and J = ≈ ¨ w ¸ 0 w e 2 ¨ ¸ (G") © M z ¹

TAINSTRUMENTS.COM )UHTXHQF\LQ'+55KHRPHWHU

DHR has a combined motor and transducer design. In an DHR rheometer, the applied motor torque and the measured amplitude are coupled. The moment of inertia required to move the motor and geometry (system inertia) is coupled with the angular displacement measurements. This means that BOTH the system inertia and the sample contributes to the measured signal.

TAINSTRUMENTS.COM ,QHUWLDO(IIHFWV

What is Inertia? Definition: That property of matter which manifests itself as a resistance to any change in momentum of a body Instrument has inertia Sample has inertia

TAINSTRUMENTS.COM ,QHUWLDO(IIHFWVLQ2VFLOODWLRQIRU'+5

Inertia consideration Viscosity limitations with frequency Minimize inertia by using low mass geometries Monitor inertia using Raw Phase in degree When Raw Phase is greater than:

150° degrees for AR series

175° degrees for DHR series

This indicates that the system inertia is dominating the measurement signal. Data may not be valid

Raw Phase × Inertia Correction = delta

TAINSTRUMENTS.COM Access to raw phase angle '+5&RUUHFWLRQIRU,QHUWLD only available with TA Instruments Rheometers!

Waveforms at high frequencies

Inertial effects at high frequencies

Negligible correction at low frequencies

TAINSTRUMENTS.COM )UHTXHQF\6ZHHSVLQ$5(6*

ARES-G2 has a separate motor and transducer design. In an ARES-G2, the motor applies the deformation independent of the torque measurement on the transducer. The moment of inertia required to move the motor is decoupled from the torque measurements. This means the motor inertia does not contribute to the test results. Benefits of ARES-G2: System inertia free Capable of running low viscosity samples up to high frequency

TAINSTRUMENTS.COM $5(6*&ORVHG/RRS&RQWURO

FRT Deflection FRT null Position Purest Measurement ! Torque to drive FRT To maintain Zero Position = Sample Torque

Motor Inertia Target NOT Part of Strain Motor Measured Measurement Displacement Or Speed

Motor torque and sample torque are Torque to separated. drive motor to desired displacement

TAINSTRUMENTS.COM '\QDPLF7HPSHUDWXUH5DPS

A linear heating rate is applied. The material response is monitored at a constant frequency and constant amplitude of deformation. Data is taken at user defined time intervals. time between data points m = ramp rate (°C/min)

Temperature (°C) Temperature Denotes Oscillatory Measurement time (min)

TAINSTRUMENTS.COM 7HPSHUDWXUH6ZHHS RU6WHS 6LQJOH0XOWL)UHTXHQF\

A step and hold temperature Soak profile is applied. The Time

material response is Step Size monitored at one, or over a

range of frequencies, at Oscillatory constant amplitude of Measurement deformation. – No thermal lag Time

Soak Time

Oscillatory Step Size Measurement

Time

TAINSTRUMENTS.COM '\QDPLF7HPSHUDWXUH5DPSRU6ZHHS0DWHULDO5HVSRQVH

Glassy Region Transition Region Rubbery Plateau Region Terminal Region

log E' (G') and (G") E" Storage Modulus (E' or G') Loss Modulus (E" or G")

dĞŵƉĞƌĂƚƵƌĞ

TAINSTRUMENTS.COM :K\ORRNDWWHPSHUDWXUHGHSHQGHQFH"

Solid in torsion rectangular

Look at Tg, secondary transitions and study structure- property relationships of finished product. Themosetting polymers Follow curing reactions Polymer melts and other liquids Measure temperature dependence of viscoelastic properties

TAINSTRUMENTS.COM $FU\ORQLWULOH%XWDGLHQH6W\UHQH $%6

TAINSTRUMENTS.COM '+5$[LDO)RUFH&RQWURO

It is important to setup normal force control during any temperature change testing or curing testing Some general suggestions for normal force control For torsion testing, set normal force in tension: 1-2N ± 0.5-1.0N For curing or any parallel plate testing, set normal force in compression: 0 ± 0.5N

TAINSTRUMENTS.COM 8VLQJ$[LDO)RUFH&RQWUROLQD7KHUPRVHWWLQJ0DWHULDO

TAINSTRUMENTS.COM 7$7HFK7LS² $[LDO)RUFH&RQWURO

Videos available at www.tainstruments.com under the Videos tab or on the TA tech tip channel of YouTube™ (ŚƚƚƉƐ͗ͬͬǁǁǁ͘ǇŽƵƚƵďĞ͘ĐŽŵͬƵƐĞƌͬddĞĐŚdŝƉƐ)

TAINSTRUMENTS.COM &XUHRU7KHUPRVHW0DWHULDOV

Cures are perhaps the most challenging experiments to conduct on rheometers as they challenge all instrument specifications both high and low. The change in modulus as a sample cures can be as large as 7-8 decades and change can occur very rapidly. AR, DHR, and ARES instruments have ways of trying to cope with such large swings in modulus AR: Non-iterative sampling (w/ Axial force control) DHR: Non-iterative sampling (w/ Axial force control) and Auto-strain (w/ Axial force active) in TRIOS v3.2 or higher ARES: Auto-strain (w/ Axial force or auto-tension active)

TAINSTRUMENTS.COM 7KHUPRVHWWLQJ3RO\PHUV

Material fully cured At start of test have a material that starts as Maximum h or G’ reached liquid, paste, pressed power Pellet, or prepreg

η Žƌ '͛

Crosslinking reaction causes h and G’ to increase

dĞŵƉ As the temp increases Material hits minimum viscosity which depends on the viscosity of resin Max temperature, frequency, ramp rate and may depend decreases on strain or stress amplitude

Time

TAINSTRUMENTS.COM '+5DQG$5'DWD&ROOHFWLRQ2SWLRQV

Non-Iterative Sampling – motor torque is adjusted based on previous stress value and predicts new value required to obtain the target strain (good for rapid measurements)

Precision Sampling – motor torque is adjusted at the end of an oscillation cycle in order to reach commanded strain

Continuous Oscillation (direct strain)* – motor torque is adjusted during the oscillation cycle to apply the commanded strain

*Continuous oscillation only available with DHR-2 and DHR-3

TAINSTRUMENTS.COM &RQWLQXRXV2VFLOODWLRQRQ6LQJOH+HDG5KHRPHWHU

Continuous oscillation (or direct strain control): incremental approach controls the strain and hits the target during a single cycle Non-iterative: uses the settings entered for the first data point and then uses previous cycle Precision: iterates using the initial settings entered for each data point

θ (t+1)1 θ (t)1

Μ (t+1)1 Μ (t)1

Point 1 or cycle

TAINSTRUMENTS.COM '+5DQG$51RQLWHUDWLYH6DPSOLQJ

η Žƌ '͛

Torque

Strain

Concern: How high does strain go at minimum Temp viscosity. Does higher strain inhibit the cure (break structure that begins to form as material crosslinks). Does this affect time to minimum viscosity or gel time?

Time

TAINSTRUMENTS.COM $5(6$5(6*DQG'+5$XWR6WUDLQ

Torque Upper torque limit

Strain

η Žƌ '͛

Temp Lower torque limit

Time

TAINSTRUMENTS.COM $[LDO)RUFH&RQWURODQG$XWRVWUDLQ

ARES-G2 DHR

TAINSTRUMENTS.COM 8VLQJ$XWR6WUDLQLQD7HPSHUDWXUH5DPS 8S

TAINSTRUMENTS.COM 8VLQJ$XWR6WUDLQLQD7HPSHUDWXUH5DPS 'RZQ

TAINSTRUMENTS.COM 7KHUPRVHW7HVWLQJ&RQVLGHUDWLRQV

Strain Depends on sample Verify the LVR in the cured state ( e.g. 0.05%) Normal force control or auto-tension Requires active to adjust for sample shrinkage and/or thermal expansion in parallel plates Temperature Isothermal Fast ramp + isotherm: the fastest ramp rate Continuous ramp rate: 3 – 5 °C/min. Frequency Typically 1Hz (6.28 rad/s), 10 rad/s or higher

TAINSTRUMENTS.COM 6HWWLQJXS5KHRORJLFDO([SHULPHQWV 7UDQVLHQW7HVWV

TAINSTRUMENTS.COM 6WUHVV5HOD[DWLRQ([SHULPHQW

Strain is applied to sample instantaneously (in principle) and held constant with time. Stress is monitored as a function of time σ(t). DHR and AR Response time dependent on feedback loop Strain

Ϭ time

TAINSTRUMENTS.COM 6WUHVV5HOD[DWLRQ([SHULPHQW

Ϭ time Response of Classical Extremes

Hookean Solid Newtonian Fluid

stress for t>0 is 0 stress for t>0 is constant Ϭ time Ϭ time

TAINSTRUMENTS.COM 6WUHVV5HOD[DWLRQ([SHULPHQW

Response of ViscoElastic Material

Stress decreases with time starting at some high value and decreasing to zero. Ϭ time

For small deformations (strains within the linear region) the ratio of stress to strain is a function of time only.

This function is a material property known as the STRESS RELAXATION MODULUS, G(t) G(t) = σ(t)/γ

TAINSTRUMENTS.COM 6WUHVV5HOD[DWLRQ0DWHULDO5HVSRQVH

Glassy Region Transition Region Rubbery Terminal Plateau Region Region

log time

TAINSTRUMENTS.COM 6WUHVV5HOD[DWLRQRQ3'06

ϭ͘ϬϬϱ

ϭϬϬϬϬ

ϭϬϬϬ

ϭϬϬ

ϭϬ

ϭ Ϭ͘Ϭϭ Ϭ͘ϭ ϭ ϭϬ ϭϬϬ time (s)

TAINSTRUMENTS.COM 'HWHUPLQLQJ6WUDLQ)RU6WUHVV5HOD[DWLRQ

Research Approach, such as generation of a family of curves for TTS, then the strain should be in the linear viscoelastic region. The stress relaxation modulus will be independent of applied strain (or will superimpose) in the linear region.

Application Approach, mimic real application. Then the question is "what is the range of strain that I can apply on the sample?" This is found by knowing the Strain range the geometry can apply. The software will calculated this for you.

γ с<γ п θ ;йγ с γ пϭϬϬͿ

TAINSTRUMENTS.COM 6WUHVV5HOD[DWLRQDQG/LQHDU5HJLRQ

Stress Relaxation of PDMS, Overlay

105 G(t) 200% strain 50% strain 10% strain 104 )

103 [Pa] G(t) ( G(t)

102

200% strain is outside the linear region 101 0.0 5.0 10.0 15.0 20.0 25.0 30.0 time [s]

TAINSTRUMENTS.COM &UHHS5HFRYHU\([SHULPHQW

Stress is applied to sample instantaneously, t1, and held constant for a specific period of time. The strain is monitored as a function of time (γ(t) or ε(t))

The stress is reduced to zero, t2, and the strain is monitored as a function of time (γ(t) or ε(t)) Native mode on AR (<1 msec) Stress

t1 time t2

TAINSTRUMENTS.COM &UHHS5HFRYHU\([SHULPHQW

t1 time t2 Response of Classical Extremes

Stain rate for t>t1 is constant Stain for t>t1 is constant Strain for t>t1 increase with time Strain for t >t2 is 0 Strain rate for t >t2 is 0

time t1 time t2 t1 t2

TAINSTRUMENTS.COM &UHHS0DWHULDO5HVSRQVH

Rubbery Plateau Region

Transition Region

Glassy Region Terminal Region log Creep Compliance, Jc Creep log ůŽŐƚŝŵĞ

TAINSTRUMENTS.COM &UHHS5HFRYHU\5HVSRQVHRI9LVFRHODVWLF 0DWHULDO

ƌĞĞƉσ хϬ

σ/η

ƚ ƚ 1 2 ƚŝŵĞ

^ƚƌĂŝŶƌĂƚĞĚĞĐƌĞĂƐĞƐ ǁŝƚŚƚŝŵĞŝŶƚŚĞĐƌĞĞƉ ǌŽŶĞ͕ƵŶƚŝůĨŝŶĂůůǇ ƌĞĂĐŚŝŶŐĂƐƚĞĂĚǇƐƚĂƚĞ͘

DĂƌŬ͕:͕͘Ğƚ͘Ăů͕͘WŚǇƐŝĐĂůWƌŽƉĞƌƚŝĞƐŽĨWŽůǇŵĞƌƐ͕ŵĞƌŝĐĂŶŚĞŵŝĐĂů^ŽĐŝĞƚǇ͕ϭϵϴϰ͕Ɖ͘ϭϬϮ͘

TAINSTRUMENTS.COM &UHHS5HFRYHU\5HVSRQVHRI9LVFRHODVWLF 0DWHULDO

ƌĞĞƉσ хϬ ZĞĐŽǀĞƌǇσ сϬ;ĂĨƚĞƌƐƚĞĂĚǇƐƚĂƚĞͿ

σ/η ZĞĐŽǀĞƌĂďůĞ ^ƚƌĂŝŶ

hŶƌĞĐŽǀĞƌĂďůĞ ^ƚƌĂŝŶ ƚ ƚ 1 2 ƚŝŵĞ

^ƚƌĂŝŶƌĂƚĞĚĞĐƌĞĂƐĞƐ /ŶƚŚĞƌĞĐŽǀĞƌǇǌŽŶĞ͕ƚŚĞǀŝƐĐŽĞůĂƐƚŝĐ ǁŝƚŚƚŝŵĞŝŶƚŚĞĐƌĞĞƉ ĨůƵŝĚƌĞĐŽŝůƐ͕ĞǀĞŶƚƵĂůůǇƌĞĂĐŚŝŶŐĂ ǌŽŶĞ͕ƵŶƚŝůĨŝŶĂůůǇ ĞƋƵŝůŝďƌŝƵŵĂƚƐŽŵĞƐŵĂůůƚŽƚĂůƐƚƌĂŝŶ ƌĞĂĐŚŝŶŐĂƐƚĞĂĚǇƐƚĂƚĞ͘ ƌĞůĂƚŝǀĞƚŽƚŚĞƐƚƌĂŝŶĂƚƵŶůŽĂĚŝŶŐ͘

DĂƌŬ͕:͕͘Ğƚ͘Ăů͕͘WŚǇƐŝĐĂůWƌŽƉĞƌƚŝĞƐŽĨWŽůǇŵĞƌƐ͕ŵĞƌŝĐĂŶŚĞŵŝĐĂů^ŽĐŝĞƚǇ͕ϭϵϴϰ͕Ɖ͘ϭϬϮ͘

TAINSTRUMENTS.COM &UHHS5HFRYHU\([SHULPHQW

Creep σ > 0 Recovery σ = 0 (after steady state)

σ/η Less Elastic

More Elastic Creep Zone Recovery Zone

t1 t2 time

TAINSTRUMENTS.COM &UHHS5HFRYHU\&UHHSDQG5HFRYHUDEOH&RPSOLDQFH

more elastic ϭͬη : Ğ Creep Zone Je = Equilibrium recoverable compliance ;ƚͿ ƌ : :;ƚͿ

Recovery Zone time time Creep Compliance Recoverable Compliance ஓሺ୲ሻ ɀ െɀ ൌ ൌ ୳ ୰ ɐ γ The material property obtained from Where u = Strain at unloading Creep experiments: γ(t) = time dependent Compliance = 1/Modulus (in a sense) recoverable strain

Mark, J., et. al., Physical Properties of Polymers, American Chemical Society, 1984, p. 102.

TAINSTRUMENTS.COM 9LVFRHODVWLF5LQJLQJ² '+5RU$5

• The ringing oscillations can be rather short-lived and may not be apparent unless using log time scale. • The sudden acceleration, together with the measurement system’s inertia, causes a strain overshoot. For viscoelastic materials, this can result in viscoelastic ringing, where the material undergoes a damped oscillation just like a bowl of Jell-o when bumped.

Creep ringing in rheometry or how to deal with oft-discarded data in step stress tests! RH Ewoldt, GH McKinley - Rheol. Bull, 2007

TAINSTRUMENTS.COM $5(6*6WUHVV&RQWURO/RRS

/ŶŶĞƌ DŽƚŽƌWŽƐŝƚŝŽŶ>ŽŽƉ σ θ ĐŵĚ;ƚͿ Δσ;ƚͿ θ;ƚͿ ;ƚͿ W/ ŵŽƚŽƌ

ŝŶƚĞŐƌĂƚŽƌ σ;ƚͿ &Zd ƐĂŵƉůĞ

>ŝŶĞĂƌƌĞƐƉŽŶƐĞ DĂƚĞƌŝĂůƌĞƐƉŽŶƐĞ

Stress is controlled by closing the loop around the sample Æ requires optimization of control PID parameters Pretest to determine material’s response and PID Constants

TAINSTRUMENTS.COM 3URJUDPPLQJ&UHHSRQDQ$5(6*

Set up a pre-test and get the sample information into the loop Stress Control Pre-test: frequency sweep within LVR

TAINSTRUMENTS.COM $5(6*6WUHVV&RQWURO3UHWHVW

Pretest Æ Frequency Sweep from 2 to 200 rad/s Æ data analyzed in software to optimize Motor loop control PID constants

LDPE melt Freq. Sweep T = 190°C

TAINSTRUMENTS.COM &UHHSRQ+'3(0HOW

3.5000 HDPE Creep Recovery at 200°C

3.0000

2.5000

2.0000

% strain 1.5000

1.0000

0.50000

0 0 2000.000 4000.000 6000.000 8000.000 10000.000 time global (s)

TAINSTRUMENTS.COM 'HWHUPLQLQJ6WUHVV)RU&UHHS([SHULPHQW

Research Approach - If you are doing creep on a polymer melt, and are interested in viscoelastic information (creep and recoverable compliance), then you need to conduct the test at a stress within the linear viscoelastic region of the material. Application Approach - If you are doing creep on a solid, you want to know the dimension change with time under a specified stress and temperature, then the questions is "what is the max/min stress that I can apply to the sample?". This is found by knowing the Stress range the geometry can apply. The software will calculated this for you.

σ = Kσ x Μ

TAINSTRUMENTS.COM $SSOLFDWLRQVRI5KHRORJ\ 3RO\PHUV

TAINSTRUMENTS.COM 3XUSRVHRID5KHRORJLFDO0HDVXUHPHQW

Three main reasons for rheological testing: Characterization MW, MWD, formulation, state of flocculation, etc. Process performance Extrusion, blow molding, pumping, leveling, etc. Product performance Strength, use temperature, dimensional stability, settling stability, etc.

TAINSTRUMENTS.COM 3RO\PHU7HVWLQJDQG5KHRORJ\

Molecular Structure MW and MWD Chain Branching and Cross-linking Interaction of Fillers with Matrix Polymer Single or Multi-Phase Structure Viscoelastic Properties As a function of: Strain Rate(frequency) Strain Amplitude Temperature Processability & Product Performance

TAINSTRUMENTS.COM 5KHRORJ\$SSOLFDWLRQVLQ3RO\PHUV

Material Property Composites, Thermosets Viscosity, Gelation, Rate of Cure, Effect of Fillers and Additives Cured Laminates Glass Transition, Modulus Damping, impact resistance, Creep, Stress Relaxation, Fiber orientation, Thermal Stability

Thermoplastics Blends, Processing effects, stability of molded parts, chemical effects

Elastomers Curing Characteristics, effect of fillers, recovery after deformation Coating, Adhesives Damping, correlations, rate of degree of cure, glass transition temperature, modulus

TAINSTRUMENTS.COM 0RVW&RPPRQ([SHULPHQWVRQ3RO\PHUV

Oscillation/Dynamic Time Sweep

Degradation studies, stability for subsequent testing Strain Sweep – Find LVER Frequency Sweep – G’, G”, η*

Sensitive to MW/MWD differences melt flow can not see Temperature Ramp/Temperature Step

Transitions, viscosity changes TTS Studies Flow/Steady Shear Viscosity vs. Shear Rate Plots Find Zero Shear Viscosity Low shear information is sensitive to MW/MWD differences melt flow can not see Creep and Recovery Creep Compliance/Recoverable Compliance Very sensitive to long chain tails

TAINSTRUMENTS.COM 3RO\PHU0HOW7KHUPDO6WDELOLW\

Polyester Temperature stability 275 Determines if properties Temperature stability are changing over the good poor time of testing 5 250 10 Degradation Molecular weight 225 building Crosslinking

Modulus G'[Pa] 200 104 Temperature T [°C]

175 -2024681012141618 Time t [min]

Important, but often overlooked!

TAINSTRUMENTS.COM ,GHDOL]HG)ORZ&XUYH² 3RO\PHU0HOWV

Power Law Region

First Newtonian Plateau η 0 = Zero Shear Viscosity η 3.4 0 = K x MW Extend Range ηη with Time- Temperature log log Superposition (TTS) Measure in Flow Mode & Cox-Merz

Extend Range Second Newtonian with Oscillation Plateau & Cox-Merz

Molecular Structure Compression Molding Extrusion Blow and Injection Molding

1.00E-5 1.00E-4 1.00E-3 0.0100 0.100 1.00 10.00 100.00 1000.00 1.00E4 1.00E5 shear rate (1/s)

TAINSTRUMENTS.COM 0HOW5KHRORJ\0:(IIHFWRQ=HUR6KHDU9LVFRVLW\

Sensitive to Molecular Weight, MW η For Low MW (no Entanglements) 0 is proportional to MW η 3.4 For MW > Critical MWc, 0 is proportional to MW

o 3.4 η MWc log

η ⋅⋅⋅ ϯ͘ϰ η с<⋅⋅⋅Dǁ 0 с< Dǁ 0 log MW

Ref. Graessley, Physical Properties of Polymers, ACS, c 1984.

TAINSTRUMENTS.COM ,QIOXHQFHRI0:RQ9LVFRVLW\

The zero shear viscosity increases with increasing molecular weight. TTS is applied to obtain the extended frequency range.

107 SBR M [g/mol] The high frequency w 130 000 behavior 106 230 000 (slope -1) is 320 000 independent of the 430 000 molecular weight 105 * [Pa s]* [Pa η

4 Zero Shear [Pas]

10 o Viscosity η

106 3 Viscosity Viscosity 10 Slope 3.08 +/- 0.39 Zero Shear Viscosity

105 2 100000 Molecilar weight M [Daltons] 10 w

10-4 10-3 10-2 10-1 100 101 102 103 104 105 Frequency ω a [rad/s] T

TAINSTRUMENTS.COM ,QIOXHQFHRI0:'RQ9LVFRVLW\

A Polymer with a broad MWD exhibits non-Newtonian flow η at a lower rate of shear than a polymer with the same 0, but has a narrow MWD.

Narrow MWD

Broad MWD

Log Shear Rate (1/s)

TAINSTRUMENTS.COM ,QIOXHQFHRI0:RQ*¶DQG*´

The G‘ and G‘‘ curves are shifted to lower frequency with increasing molecular weight.

106

105

104 SBR M [g/mol] w 3 G' 130 000 10 G'' 130 000 G' 430 000

Modulus G', G'' [Pa] Modulus 2 G'' 430 000 10 G' 230 000 G'' 230 000 101 10-4 10-3 10-2 10-1 100 101 102 103 104 105 Freq ω [rad/s]

TAINSTRUMENTS.COM ,QIOXHQFHRI0:'RQ*¶DQG*´

106

105 The maximum in G‘‘ is a good indicator of the broadness of the 104 distribution SBR polymer melt G' 310 000 broad Modulus G',Modulus G'' [Pa] 3 G" 310 000 broad 10 G' 320 000 narrow G" 320 000 narrow EĂƌƌŽǁ -3 -2 -1 0 1 2 3 4 10 10 10 10 10 10 10 10 ƌŽĂĚ Frequency ωa [rad/s] T

Higher crossover frequency : lower Mw Higher crossover Modulus: narrower MWD (note also the slope of G” at low frequencies – narrow MWD steeper slope)

TAINSTRUMENTS.COM +LJK0:&RQWULEXWLRQV

400,000 g/mol PS 400,000 g/mol PS 400,000 g/mol PS + 1% 12,000,000 g/mol + 4% 12,000,000 g/mol

Macosko, TA Instruments Users’ Meeting, 2015 TAINSTRUMENTS.COM ,PSRUWDQFHRI9HULI\LQJ7KHUPDO6WDELOLW\

Good thermal stability one crossover point, Ș* plateaus at low Ȧ

Poor thermal stability multiple crossover points Ș* continues to increase over time Time Sweep can verify if the sample is unstable

TAINSTRUMENTS.COM 6XUIDFH'HIHFWVGXULQJ3LSH([WUXVLRQ

HDPE pipe surface defects

o Surface roughness T = 220 C 5 5 correlates with G‘ or 10 10 elasticity → broader MWD or tiny amounts of a high * [Pa s] * [Pa η MW component 4 10 104

G' rough surface Modulus G' [Pa] G' Modulus 3 G' smooth surface 10 103

η* rough surface viscosity Complex η* smooth surface

0.1 1 10 100 Frequency ω [rad/s]

Blue-labled sample shows a rough surface after extrusion

TAINSTRUMENTS.COM 7DFNDQG3HHORI$GKHVLYHV

Tack and Peel performance of a PSA

Bond strength is obained from peel good tack and peel (fast) and tack Bad tack and peel (slow) tests 104 It can be related to the viscoelastic properties at peel different frequencies 103

Storage Modulus G' [Pa] Modulus Storage tack

0.1 1 10 Frequency ω [rad/s] Tack and peel have to be balanced for an ideal adhesive

TAINSTRUMENTS.COM 'ULHG$GKHVLYHV 7DFN7HVW

TAINSTRUMENTS.COM &UHHS DQG5HFRYHU\ZLWK,QFUHDVLQJ6WUHVV

LDPE Melt creep recovery

-1 10 10-1 LDPE Melt Non linear effects 10 Pa T=140 oC 50 Pa can be detected in -2 slope 1 recovery before 10 100 Pa 10-2 500 Pa they are seen in the 1000 Pa increasing creep (viscosity stress -3 5000 Pa dominates) 10 10-3

-4 10 10-4 Compliance J(t)[1/Pa]

-5 Compliance Recoverable Jr(t)[1/Pa] 10 10-5 0.1 1 10 100 1000 Time t [s]

TAINSTRUMENTS.COM (IIHFWRI)LOOHURQ0HOW9LVFRVLW\

Neat and Filled LDPE

7 &ŝůůĞƌƐŝŶĐƌĞĂƐĞƚŚĞ 10 o Temperature 180 C ŵĞůƚǀŝƐĐŽƐŝƚǇ LDPE filled 106 LDPE neat ƵĞƚŽŝŶƚĞƌͲƉĂƌƚŝĐůĞ ŝŶƚĞƌĂĐƚŝŽŶƐ͕ƚŚĞ 105 . s] ) [Pa γ ŶŽŶͲEĞǁƚŽŶŝĂŶ ( η ƌĂŶŐĞŝƐĞǆƚĞŶĚĞĚƚŽ 4 10 ůŽǁƐŚĞĂƌƌĂƚĞƐĂŶĚ ƚŚĞǌĞƌŽƐŚĞĂƌ Viscosity Viscosity 103 ǀŝƐĐŽƐŝƚǇŝŶĐƌĞĂƐĞƐ ĚƌĂŵĂƚŝĐĂůůǇ 102 1E-5 1E-4 1E-3 0.01 0.1 1 10 100 1000 10000 . Shear rate γ [1/s]

The material has a yield, when rate and viscosity are inverse proportional at low rate.

TAINSTRUMENTS.COM ([WHQVLRQDO9LVFRVLW\0HDVXUHPHQWV

Fix drum connected to transducer

Rotating drum connected to the motor: rotates around its axis rotates around axis of fixed drum

TAINSTRUMENTS.COM :K\LV(ORQJDWLRQ9LVFRVLW\,PSRUWDQW"

Application to processing: many processing flows are elongation flows - testing as close as possible to processing conditions (spinning, coating, spraying)

Relation to material structure: non linear elongation flow is more sensitive for some structure elements than shear flows (branching, polymer architecture)

Testing of constitutive equations: elongation results in addition to shear data provide a more general picture for developing material equations

TAINSTRUMENTS.COM //'3( /RZEUDQFKLQJ

η

TAINSTRUMENTS.COM /'3( +LJKEUDQFKLQJ

η

TAINSTRUMENTS.COM 7KHUPRVHWWLQJ3RO\PHUV

Thermosetting polymers are perhaps the most challenging samples to analyze on rheometers as they challenge all instrument specifications both high and low.

The change in modulus as a sample cures can be as large as 7-8 decades and change can occur very rapidly.

TAINSTRUMENTS.COM 7KHUPRVHWV$QDO\VLV

Monitor the curing process Viscosity change as function of time or temperature Gel time or temperature Test methods for monitoring curing Temperature ramp Isothermal time sweep Combination profile to mimic process Analyze cured material’s mechanical properties (G’, δ G”, tan , Tg etc.)

TAINSTRUMENTS.COM 6WUXFWXUDO'HYHORSPHQW'XULQJ&XULQJ

'ĞůƉŽŝŶƚ

TAINSTRUMENTS.COM $WWKH*HO3RLQW

Molecular weight Mw goes to infinity System loses solubility Zero shear viscosity goes to infinity Equilibrium Modulus is zero and starts to rise to a finite number beyond the gel point

Note: For most applications, gel point can be considered as when G’ = G” and tan δ = 1

TAINSTRUMENTS.COM &XULQJ$QDO\VLV,VRWKHUPDO&XULQJ

TA Instruments 1000000 G' 1000000 5 min 100000 100000

10000 G" 10000 G'' (Pa)

1000 1000

G' (Pa) Gel Point: G' = G" t = 330 s 100.0 100.0

10.00 10.00

1.000 1.000 0 200.0 400.0 600.0 800.0 1000 1200 time (s)

TAINSTRUMENTS.COM 7KHUPRVHW8VLQJD7HPSHUDWXUH5DPS

^ƵƌĨĂĐĞDĂƐƚĞƌ® ϵϬϱ

TAINSTRUMENTS.COM $WWKH*HO3RLQW&RQWLQXHG«

• The process of viscosity increasing takes place in two stages: the gelation process (frequency independent) and vitrification (related to the network Tg relative to cure temperature and is frequency dependent). • When you look at an isothermal cure at a constant frequency the modulus crossover point has both the information of gelation and vitrification. To avoid this, run multiple isothermal runs at different frequencies and plot the cross over in tan delta. This is the frequency independent gel point.

Alternatively, use a single mutliwave test

TAINSTRUMENTS.COM *HO3RLQWXVLQJ7DQ'HOWD

TAINSTRUMENTS.COM ,VRWKHUPDO&XULQJ

135°C 130°C 140°C 120°C 125°C 145°C G’ (MPa) G’

Tire Compound: Effect of Curing Temperature

Time (min)

TAINSTRUMENTS.COM 89/LJKW*XLGH&XULQJ$FFHVVRU\

Collimated light and mirror assembly insure uniform irradiance Maximum intensity at plate 300 mW/cm2 Broad range spectrum with main peak at 365 nm Cover with nitrogen purge ports Optional disposable acrylic plates

TAINSTRUMENTS.COM 89&XUH3URILOH&KDQJHVZLWK7HPSHUDWXUH

ƵƉƚŽϱϬƉŽŝŶƚƐ ƉĞƌƐĞĐŽŶĚ

TAINSTRUMENTS.COM 3RO\PHU6WUXFWXUH3URSHUW\&KDUDFWHUL]DWLRQ

Glass transition Secondary transitions Crystallinity Molecular weight/cross-linking Phase separation (polymer blends, copolymers,...) Composites Aging (physical and chemical) Curing of networks Orientation Effect of additives

Reference: Turi, Edith, A, Thermal Characterization of Polymeric Materials, Second Edition, Volume I., Academic Press, Brooklyn, New York, P. 489.

TAINSTRUMENTS.COM +RZWR0HDVXUH*ODVV7UDQVLWLRQ

G' Onset: Occurs at lowest temperature - Relates to mechanical failure

G" Peak: Occurs at middle temperature - more closely related to the physical property changes attributed to the glass transition in plastics. It reflects molecular processes -

agrees with the idea of Tg as the temperature at the onset of segmental motion. tan δ Peak: Occurs at highest temperature - used historically in literature - a good measure of the "leatherlike" midpoint between the glassy and rubbery states - height and shape change systematically with amorphous content.

Reference: Turi, Edith, A, Thermal Characterization of Polymeric Materials, Second Edition, Volume I., Academic Press, Brooklyn, New York, P. 980.

TAINSTRUMENTS.COM 3DVWD&RRNHGLQ7RUVLRQ,PPHUVLRQ

Allows samples to be Addition of Water characterized while fully 1.000E10 100.0 immersed in a temperature controlled fluid using Peltier Isotherm with 90.0 Concentric Cylinder Jacket water at 22 °C Isotherm 1.000E9 Track changes in mechanical with water 80.0 properties such as swelling or at 95 °C plasticizing

70.0 1.000E8 temperature (°C)

Temperature 60.0 G' (Pa) ramp to 95 °C G’ (Pa) G’ 1.000E7 50.0

40.0

1.000E6

30.0

1.000E5 20.0 0 10.0 20.0 30.0 40.0 50.0 60.0 timetime global (min) (min)

TAINSTRUMENTS.COM 7HVWLQJ6ROLGVRQD5KHRPHWHU

Torsion and DMA geometries allow solid samples to be characterized in a temperature controlled environment – DMA functionality is standard with ARES G2 and optional DHR

сϮ';ϭнʆͿ ʆ ͗WŽŝƐƐŽŶ͛ƐƌĂƚŝŽ

Modulus: G’, G”, G* Modulus: E’, E”, E*

Rectangular and DMA 3-point bending and tension cylindrical torsion (Cantilever not shown)

TAINSTRUMENTS.COM *ODVV7UDQVLWLRQ $%6

TAINSTRUMENTS.COM 7KH*ODVV 6HFRQGDU\7UDQVLWLRQV

Glass Transition - Cooperative motion among a large number of chain segments, including those from neighboring polymer chains

Secondary Transitions Local main-chain motion - intramolecular rotational motion of main chain segments four to six atoms in length Side group motion with some cooperative motion from the main chain Internal motion within a side group without interference from side group Motion of or within a small molecule or diluent dissolved in the polymer (e.g. plasticizer)

Reference: Turi, Edith, A, Thermal Characterization of Polymeric Materials, Second Edition, Volume I., Academic Press, Brooklyn, New York, P. 487.

TAINSTRUMENTS.COM 3RO\FDUERQDWHLQ7RUVLRQ

TAINSTRUMENTS.COM &U\VWDOOLQLW\0ROHFXODU:HLJKWDQG&URVVOLQNLQJ

Increasing Crystallinity

Amorphous Crystalline log Modulus 3 decade drop Cross-linked

in modulus at Tg

Increasing MW Tm Temperature

TAINSTRUMENTS.COM $SSOLFDWLRQVRI5KHRORJ\ 6WUXFWXUHG)OXLGV

TAINSTRUMENTS.COM 6WUXFWXUHG)OXLGV

Multiphase systems consisting of a dispersed phase (solid, fluid, gas) in surrounding fluid phase

Examples are: Properties: Paints Yield Stress Coatings Non-Newtonian Inks Viscous Behavior Personal Care Products Thixotropy Cosmetics Elasticity Foods

TAINSTRUMENTS.COM ,GHDOL]HG)ORZ&XUYH

What shear rate?

4) Chewing, swallowing 8) Spraying and brushing 1) Sedimentation 5) Dip coating 9) Rubbing 2) Leveling, Sagging 6) Mixing, stirring 10) Milling pigments 3) Draining under gravity

η 7) Pipe flow 11) High Speed coating log

4 5 6 8 9 1 2 3 7 10 11

1.00E-5 1.00E-4 1.00E-3 0.0100 0.100 1.00 10.00 100.00 1000.00 1.00E4 1.00E5 1.00E6

shear rate (1/s)

TAINSTRUMENTS.COM *HQHUDO9LVFRVLW\&XUYHIRU6XVSHQVLRQV

This viscosity is often called η the Zero Shear Viscosity, 0, or the Newtonian Viscosity

First Newtonian η Plateau Possible log Increase in Second Viscosity Power-Law Newtonian Shear Thinning Plateau

σ∝ߛሶ m or, equivalently, η∝ߛሶ m-1 m is usually 0.15 to 0.6 log ߛሶ

Reference:Barnes, H.A., Hutton, J.F., and Walters, K., An Introduction to Rheology, Elsevier Science B.V., 1989. ISBN 0-444-87469-0

TAINSTRUMENTS.COM 5HDVRQIRU6KDSHRI*HQHUDO)ORZ&XUYH

Brownian diffusion randomizes

Shear field aligns particles along η streamlines Turbulent flow pushes ůŽŐ particles out of alignment, destroying order and causing increase in viscosity (shear thickening)

Shear thinning Shear thickening

TAINSTRUMENTS.COM &ORVLQJ WKH*DS

Linear or Exponential speed profile after reaching ‘Closure Distance’ Normal Force set not to exceed a certain value after reaching the user defined ‘Closure Distance’

TAINSTRUMENTS.COM &RPSDULVRQRI/LQHDUDQG([SRQHQWLDO&ORVLQJ

ϮϱϬ Exponential Close ϮϬϬ

ϭϱϬ Fast Linear Close G' (Pa) ϭϬϬ

ϱϬ

Ϭ Ϭ ϮϬϬ ϰϬϬ ϲϬϬ ϴϬϬ ϭϬϬϬ Time (s) Lowering the gap can introduce shear, breaking down weakly structured samples Reducing the gap closure speed can minimize this effect

TAINSTRUMENTS.COM 8VLQJ3UH6KHDULQJ

Monitor the viscosity signal during the pre-shear to determine if the rate and duration are appropriate If the viscosity is increasing during the pre-shear, the sample is rebuilding. The pre-shear should be higher than the shear introduced during loading to erase sample loading history The viscosity should decrease and then level off Typical Pre-Shear: 1- 100 sec-1, 30-60 seconds Use an amplitude sweep to determine what strain to use for time sweep A high strain will break down the sample, and not allow rebuilding A low strain will give a weak signal Based on the Time Sweep, determine an appropriate equilibration time for that sample

TAINSTRUMENTS.COM 3UHVKHDU&RQGLWLRQV

The goal for pre-shear is to remove the sample history at loading For high viscosity sample, use low rate (10 1/s) and long time (2 min.) For low viscosity sample, use high rate (100 1/s) and short time (1 min.)

TAINSTRUMENTS.COM 6WUXFWXUHG)OXLG3UHWHVWLQJ

1. 2. 3.

Three consecutive time sweeps: Time sweep within LVR (check if loading destroyed structure) Time sweep at large strain Time sweep back to LVR (check structure rebuild)

TAINSTRUMENTS.COM 7LPH6ZHHSV +DQG&UHDP

^ƚŽƌĂŐĞƉƉůŝĐĂƚŝŽŶ ƚZĞƐƚ

TAINSTRUMENTS.COM

Structured fluids exhibit yield-like behavior, changing from ‘solid-like’ to readily flowing fluid when a critical stress is exceeded. Rheological modifiers are often used to control the yield behavior of fluids.

There are multiple methods to measure Yield stress. The apparent yield stress measured is not a single value, as it will vary depending on experimental conditions.

Why modify the yield behavior? to avoid sedimentation and increase the shelf live to reduce flow under gravity to stabilize a fluid against vibration

TAINSTRUMENTS.COM

Stress is ramped linearly from 0 to a value above Yield Stress and the stress at viscosity maximum can be recorded as Yield Stress The measured yield value will depend on the rate at which the stress is increased. The faster the rate of stress increase, the higher the measured yield value

TAINSTRUMENTS.COM

Yield Stress

TAINSTRUMENTS.COM

When the Yield Stress is small, a flow rate sweep from high to low shear rate is preferred

Eliminates start-up effects for more accurate measurements

slope: -0.995 Initial high shear rate acts as a pre-shear, erasing loading effects

Steady State sensing allows the sample time to rebuild

The plateau in shear stress is a measure of the yield stress.

At the plateau, Viscosity vs. Shear Rate will have a slope of -1

TAINSTRUMENTS.COM

1000 Perform strain or stress Sun Block Lotion sweep in oscillation

Yield stress is the on set of G’ curve. It is the critical

G' (Pa) stress at which irreversible Onset point osc. stress: 1.477 Pa plastic deformation occurs. G': 346.6 Pa End condition: Finished normally

100.0 0.01000 0.1000 1.000 10.00 osc. stress (Pa)

Yield stress of a sun block lotion

TAINSTRUMENTS.COM 9LVFRVLW\5DQJHVRI3DLQWV&RDWLQJV

Low shear viscosity 10-3 to 1 s-1 leveling, sagging, sedimentation

Medium shear viscosity10-103 s-1 mixing, pumping and pouring

High shear viscosity 103 -106 s-1 brushing, rolling spraying

TAINSTRUMENTS.COM 9LVFRVLW\5DQJHVRI3DLQWV&RDWLQJV

104 At Rest Processing Performance

103 LSV MSV HSV 102 Roling

1 Brushing [Pas] 10 Spraying h 100 Mixing -1 Leveling 10 Pumping Viscosity Viscosity Sagging Consistency 10-2 Sedimentation Appearence

10-3 0.1 1 10 100 1000 10000 100000 shear rate g [1/s]

The two coatings show the same consistency after formulation, but they exhibit very different application performance

TAINSTRUMENTS.COM 7KL[RWURS\

The thixotropy characterizes the time dependence of reversible structure changes in complex fluids. The control of thixotropy is important to control:

process conditions for example to avoid structure build up in pipes at low pumping rates i.e. rest periods, etc....

sagging and leveling and the related gloss of paints and coatings, etc..

Sag Leveling

TAINSTRUMENTS.COM 7KL[RWURSLF/RRS7HVW

Stress is ramped up linearly, and then back down, over the same duration

In a thixotropic material, there will be a hysterisis between the two curves

The further the up ramp and down ramp curves differ, the larger the area between the curves, the higher the thixotropy of the material. See also AAN 016 – Structured Fluids

TAINSTRUMENTS.COM 6WUXFWXUH5HFRYHU\

after preshear η* Structure build up G'

* [Pas] G'' Pre-shear the sample η 102 G' to break down oo structure. Then monitor the increase of the modulus or complex viscosity as Frequency 1Hz G' strain 2% function of time. o preshear 10s at 60 s-1 Modulus G', G'' [Pa]; Viscosity Viscosity G'' [Pa]; Modulus G',

0 20406080100120 time t min]

ᇱ ௧Ȁఛ τ Ԣሻሺͳ െ ݁ ) = characteristic recovery timeܩԢஶ െܩԢ ሺܩݐൌ ܩ

TAINSTRUMENTS.COM 7LPH6ZHHSDIWHU3UH6KHDULQJ

ᇱ ௧Ȁఛ ( ݁ Ԣሻሺͳ െܩԢஶ െܩԢ ሺܩݐൌ ܩ ͛ Ăс' ĂƚƚŝŵĞǌĞƌŽ;ƚϬͿ ͛ ďс' ĂƚŝŶĨŝŶŝƚĞƚŝŵĞ;ƚ∞Ϳ ĐсĐŚĂƌĂĐƚĞƌŝƐƚŝĐƌĞĐŽǀĞƌǇƚŝŵĞ;τͿ

TAINSTRUMENTS.COM 7KL[RWURSLF,QGH[ 5HFRYHU\7LPH

The non-sagging formula (with additive) has both a shorter recovery time and a higher final recovered viscosity (or storage modulus), and the recovery parameter takes both of these into account to predict significantly better sag resistance.

The ratio η(∞) /t, is the recovery parameter (a true thixotropic index), and has been found to correlate well to thixotropy-related properties such as sag resistance and air entrainment.

Rheology in coatings, principles and methods RR Eley - Encyclopedia of Analytical Chemistry, 2000 - Wiley Online Library

TAINSTRUMENTS.COM &DVH6WXG\RI3DLQWV

100.0

Paint A

10.00 Paint B

Paint C viscosity (Pa.s)

1.000 Paint D

0.1000 0.01000 0.1000 1.000 10.00 100.0 shear rate (1/s)

TAINSTRUMENTS.COM &DVH6WXG\RI3DLQWV

120.0 Thixotropy (Pa/s): Paint A = 657.0 Paint B = 436.5 100.0 Paint C = 254.0 Paint D = 120.3

80.00

Paint A

60.00 shear stress (Pa)

Paint B 40.00

Paint C

20.00

Paint D

0 0 10.00 20.00 30.00 40.00 50.00 60.00 70.00 80.00 90.00 100.0 shear rate (1/s)

TAINSTRUMENTS.COM &DVH6WXG\RI3DLQWV

15.00

Paint A

12.50

10.00

7.500 G' (Pa)

5.000 Paint B

2.500 Paint C

Paint D

0 0 100.0 200.0 300.0 400.0 500.0 600.0 700.0 800.0 900.0 time (s)

TAINSTRUMENTS.COM &DVH6WXG\RI3DLQWV

Paint A Paint B

Paint C Paint D

TAINSTRUMENTS.COM $QWLSHUVSLUDQW'HRGRUDQW

Roll-ons: Rheology and end-use performance The viscosity has to be balanced to provide the correct viscosity at a given shear rate

storage viscosity application

shear rate

TAINSTRUMENTS.COM $QWLSHUVSLUDQW'HRGRUDQW

Sticks: Rheology and process performance

use small particles to reduce sedimentation speed

add rheological modifier like clay to stabilize the suspension and keep the particles in suspension

ϭнϬϴ x x x x x x x ϭнϬϳ x The temperature x ϭнϬϲ x dependence of the modulus governs the ϭнϬϱ x behavior during the ϭнϬϰ x application to the skin DŽĚƵůƵƐ'ΖWĂ ϭнϬϯ Ϭ ϭϬϮϬϯϬϰϬϱϬϲϬϳϬ dĞŵƉĞƌĂƚƵƌĞ

TAINSTRUMENTS.COM (ODVWLFLW\2VFLOODWLRQ)UHTXHQF\6ZHHS

Cosmetic lotion Many dispersion exhibit 2.0 solid like behavior at rest 103 1.5 * [Pa s] * [Pa η The frequency 1.0 dependence and the δ 102 0.5 δ absolute value of tan correlate with long time tan tan 0.0 stability complex viscosity

G' -0.5 101 G'' tan δ -1.0 Modulus G', G'' [Pa]; Modulus Viscosity 0.1 1 10 100 frequency ω [rad/s]

Note: strain amplitude has to be in the linear region

TAINSTRUMENTS.COM )RDP+DQGZDVK 6WUDLQ6ZHHS'LQYV9DQH5RWRU

DIN Vane

TAINSTRUMENTS.COM 75,26+HOS0HQX

Browse the contents list or search using the search tab.

Access to Getting Started Guides also found through the help menu.

TAINSTRUMENTS.COM ,QVWUXFWLRQDO9LGHRV

From www.tainstruments.com click on Videos, Support or Training

Select Videos for TA Tech Tips, Webinars and Quick Start Courses

^ĞĞĂůƐŽ͗ŚƚƚƉƐ͗ͬͬǁǁǁ͘ǇŽƵƚƵďĞ͘ĐŽŵͬƵƐĞƌͬddĞĐŚdŝƉƐ

TAINSTRUMENTS.COM ,QVWUXFWLRQDO9LGHR5HVRXUFHV

Quickstart e-Training Courses Strategies for Better Data - Rheology

TAINSTRUMENTS.COM 1HHG$VVLVWDQFH"

Check the online manuals and error help. Contact the TA Instruments Hotline Phone: 302-427-4070 M-F 8-4:30 EST Select Thermal , Rheology or Microcalorimetry Support Email: [email protected] or [email protected] or [email protected] Call your local Technical or Service Representative Call TA Instruments Phone: 302-427-4000 M-F 8-4:30 EST Check out our Website: www.tainstruments.com For instructional videos go to: www.youtube.com/user/TATechTips

TAINSTRUMENTS.COM Thank You

The World Leader in Thermal Analysis, Rheology, and Microcalorimetry

TAINSTRUMENTS.COM $SSHQGL[7LPH7HPSHUDWXUH 6XSHUSRVLWLRQ 776

TAINSTRUMENTS.COM 7LPHDQG7HPSHUDWXUH 5HODWLRQVKLS

(E' or G') (E' or G') (E" or G") (E" or G")

log Frequency Temperature Linear viscoelastic properties are both time-dependent and temperature-dependent Some materials show a time dependence that is proportional to the temperature dependence Decreasing temperature has the same effect on viscoelastic properties as increasing the frequency For such materials, changes in temperature can be used to “re-scale” time, and predict behavior over time scales not easily measured

TAINSTRUMENTS.COM 7LPH7HPSHUDWXUH6XSHUSRVLWLRQLQJ%HQHILWV

TTS can be used to extend the frequency beyond the instrument’s range Creep TTS or Stress Relaxation TTS can predict behavior over longer times than can be practically measured Can be applied to amorphous, non modified polymers Material must be thermo-rheological simple

One in which all relaxations times shift with the same shift factor aT

TAINSTRUMENTS.COM :KHQ1RWWR8VH776

If crystallinity is present, especially if any melting occurs in the temperature range of interest

The structure changes with temperature

Cross linking, decomposition, etc.

Material is a block copolymer (TTS may work within a limited temperature range)

Material is a composite of different polymers

Viscoelastic mechanisms other than configuration changes of the polymer backbone

e.g. side-group motions, especially near the Tg

Dilute polymer solutions

Dispersions (wide frequency range)

Sol-gel transition

TAINSTRUMENTS.COM *XLGHOLQHVIRU776

Decide first on the Reference Temperature: T0. What is the use temperature?

If you want to obtain information at higher frequencies or shorter times, you will need to conduct frequency (stress

relaxation or creep) scans at temperatures lower than T0.

If you want to obtain information at lower frequencies or longer times, you will need to test at temperatures higher

than T0.

Good idea to scan material over temperature range at single frequency to get an idea of modulus-temperature and transition behavior.

TAINSTRUMENTS.COM 7766KLIWLQJ

TAINSTRUMENTS.COM 7766KLIWLQJ

TAINSTRUMENTS.COM 7766KLIWLQJ

TAINSTRUMENTS.COM 7766KLIWLQJ

TAINSTRUMENTS.COM 7766KLIWLQJ

TAINSTRUMENTS.COM 7766KLIWLQJ

TAINSTRUMENTS.COM 7766KLIWLQJ

aT=140

aT=150

aT=160

TAINSTRUMENTS.COM 6KLIW)DFWRUVD7 YV7HPSHUDWXUH

TAINSTRUMENTS.COM 6KLIW)DFWRUV:/)(TXDWLRQ

Master Curves can be generated using shift factors derived from the Williams, Landel, Ferry (WLF) equation

log aT= -c1(T-T0)/c2+(T-T0)

aT = temperature shift factor

T0 = reference temperature

c1 and c2 = constants from curve fitting

Generally, c1=17.44 & c2=51.6 when T0 = Tg

TAINSTRUMENTS.COM :KHQQRWWRXVHWKH:/)(TXDWLRQ

Sometimes you shouldn’t use the WLF equation (even if it appears to work)

If T > Tg+100°C If T < Tg and polymer is not elastomeric If temperature range is small, then c1 & c2 cannot be calculated precisely

In these cases, the Arrhenius form is usually better

ln aT = (Ea/R)(1/T-1/T0)

aT = temperature shift factor Ea = Apparent activation energy T0 = reference temperature T = absolute temperature

R = gas constant

Ea = activation energy

TAINSTRUMENTS.COM 9HULI\'DWDIRU776

Polystryene

TAINSTRUMENTS.COM 9HULI\'DWDIRU776

Polystryene

TAINSTRUMENTS.COM 5HIHUHQFHVIRU776

1) Ward, I.M. and Hadley, D.W., "Mechanical Properties of Solid Polymers", Wiley, 1993, Chapter 6.

2) Ferry, J.D., "Viscoelastic Properties of Polymers", Wiley, 1970, Chapter 11.

3) Plazek, D.J., "Oh, Thermorheological Simplicity, wherefore art thou?" Journal of Rheology, vol 40, 1996, p987.

4) Lesueur, D., Gerard, J-F., Claudy, P., Letoffe, J-M. and Planche, D., "A structure related model to describe asphalt linear viscoelasticity", Journal of Rheology, vol 40, 1996, p813.

TAINSTRUMENTS.COM $SSHQGL[6RIWZDUH6FUHHQ6KRWV 75,26

TAINSTRUMENTS.COM '+53HDN+ROG&RQVWDQW6KHDU5DWHYV7LPH

TAINSTRUMENTS.COM $5(6*6WUHVV*URZWK7HVW 6WHS5DWH

TAINSTRUMENTS.COM &RQWLQXRXV5DPS

Control variables: Shear rate Velocity Torque Shear stress

Thixotropic loop be done by adding another ramp step

TAINSTRUMENTS.COM Thixotropic loop

TAINSTRUMENTS.COM $5(6*6WUHVV5DPS6WUHVV&RQWURO3UHWHVW

TAINSTRUMENTS.COM $5(6*6WUHVV5DPS 7KL[RWURSLF/RRS

TAINSTRUMENTS.COM '+5DQG$5(6*6WHDG\6WDWH)ORZ

Control variables: Shear rate Velocity Torque Shear stress

Steady state algorithm

TAINSTRUMENTS.COM '+5DQG$5(6*)ORZ7HPS5DPS

To minimize thermal lag, the ramp rate should be slow. 1-5°C/min.

Control variables: Shear rate Velocity Torque Shear stress

TAINSTRUMENTS.COM '+56WUDLQ6WUHVV6ZHHSV

Control variables: Osc torque Osc stress Displacement % strain Strain

TAINSTRUMENTS.COM $5(6*6WUDLQ6ZHHS

TAINSTRUMENTS.COM '+57LPH6ZHHS

Pre-shear can be setup by adding a “conditioning” step before the time sweep.

The strain needs to be in the LVR

TAINSTRUMENTS.COM $5(6*7LPH6ZHHS

Pre-shear step

Structure Recovery

TAINSTRUMENTS.COM )DVW'DWD6DPSOLQJ2SWLRQLQ7LPH6ZHHS

Strain control mode Stress control mode

Fast data acquisition is used for monitoring fast changing reactions such as UV initiated curing The sampling rate for this mode is twice the functional oscillation frequency up to 25Hz. The fastest sampling rate is 50 points /sec.

TAINSTRUMENTS.COM )UHTXHQF\6ZHHS

Control variables: Osc torque Osc stress Displacement % strain Strain

Common frequency range: 0.1 – 100 rad/s. Low frequency takes long time As long as in the LVR, the test frequency can be set either from high to low, or low to high The benefit doing the test from high to low Being able to see the initial data points earlier

TAINSTRUMENTS.COM $5(6*)UHTXHQF\6ZHHS 6WUDLQ&RQWURO

TAINSTRUMENTS.COM '+57HPSHUDWXUH6ZHHS

Control variables: Osc torque Osc stress Displacement % strain Strain

The strain needs to be in the LVR

TAINSTRUMENTS.COM '+57HPSHUDWXUH5DPS

To minimize thermal lag, recommend using slow ramp rate e.g. 1-5°C/min.

The strain needs Control variables: to be in the LVR Osc torque Osc stress Displacement % strain Strain

TAINSTRUMENTS.COM '+5$[LDO)RUFH&RQWURO

It is important to setup normal force control during any temperature change testing or curing testing Some general suggestions for normal force control For torsion testing, set normal force in tension: 1-2N ± 0.5-1.0N For curing or any parallel plate testing, set normal force in compression: 0 ± 0.5N

TAINSTRUMENTS.COM $5(6*7HPS6WHS

TAINSTRUMENTS.COM $5(6*7HPS5DPS

TAINSTRUMENTS.COM $5(6*$[LDOIRUFHFRQWURODQGDXWRVWUDLQ

TAINSTRUMENTS.COM '+56WUHVV5HOD[DWLRQ

TAINSTRUMENTS.COM $5(6*6WUHVV5HOD[DWLRQ

TAINSTRUMENTS.COM '+5&UHHS5HFRYHU\

Creep Recovery

Rule of thumb: recovery time is 2-3 times longer than creep time

TAINSTRUMENTS.COM $5(6*&UHHS

Requires measured modulus to start feed back loop

Motor and transducer work in a feedback loop

TAINSTRUMENTS.COM 3URJUDPPLQJ&UHHSRQD$5(6*

Set up a pre-test and get the sample information into the loop Stress Control Pre-test: frequency sweep within LVR

TAINSTRUMENTS.COM $5(6*&UHHS 5HFRYHU\

TAINSTRUMENTS.COM $SSHQGL[6RIWZDUH6FUHHQ6KRWV 5KHRORJ\$GYDQWDJH

TAINSTRUMENTS.COM $53HDN+ROG

Control variables: Shear rate Velocity Torque Shear stress

Multiple rate can be done by adding more peak hold steps

TAINSTRUMENTS.COM $5&RQWLQXRXV5DPS

Control variables: Shear rate Velocity Torque Shear stress

Thixotropic loop be done by adding another ramp step Or go through the template

TAINSTRUMENTS.COM $5&RQWLQXRXV5DPS

TAINSTRUMENTS.COM $56WHSSHG)ORZ

Control variables: Shear rate Velocity Torque Shear stress

TAINSTRUMENTS.COM $56WHDG\6WDWH)ORZ

Control variables: Shear rate Velocity Torque Shear stress

Steady state algorithm

During the test, the dependent variable (speed in controlled stress mode or torque in controlled shear rate mode) is monitored with time to determine when stability has been reached. An average value for the dependent variable is recorded over the Sample period. When consecutive average values (Consecutive within tolerance) are within the Percentage tolerance specified here, the data is accepted. The software will also accept the point at the end of the Maximum point time, should the data still not be at a steady state value.

TAINSTRUMENTS.COM $5)ORZ7HPS5DPS

To minimize thermal lag, the ramp rate should be slow. 1-5°C/min.

Control variables: Shear rate Velocity Torque Shear stress

TAINSTRUMENTS.COM $56WUHVV6ZHHS

Variables: Stress Torque

For running an unknown sample, it is recommended to sweep torque instead of stress. Because stress is geometry dependent The starting torque can be from the lowest of the instrument specification The maximum torque is sample dependent. You can setup a high number and manually stop the test when it gets outside the LVR.

TAINSTRUMENTS.COM $57LPH6ZHHS

Control variables: Osc torque Osc stress Displacement % strain Strain

The strain needs to be in the LVR

TAINSTRUMENTS.COM $53UHVKHDU&RQGLWLRQV

The goal for pre-shear is to remove the sample history at loading For high viscosity sample, use low rate (10 1/s) and long time (2 min.) For low viscosity sample, use high rate (100 1/s) and short time (1 min.)

TAINSTRUMENTS.COM $5)UHTXHQF\6ZHHS

Control variables: Osc torque Osc stress Displacement % strain Strain

Common frequency range: 0.1 – 100 rad/s. Low frequency takes long time As long as in the LVR, the test frequency can be set either from high to low, or low to high The benefit doing the test from high to low Being able to see the initial data points earlier

TAINSTRUMENTS.COM $57HPS6ZHHS

Control variables: Osc torque Osc stress Displacement % strain Strain

The strain needs to be in the LVR

TAINSTRUMENTS.COM $57HPS5DPS

To minimize thermal lag, recommend using slow ramp rate e.g. 1-5°C/min.

Control variables: Osc torque Osc stress Displacement % strain The strain needs to be in the LVR Strain

TAINSTRUMENTS.COM $51RUPDO)RUFH&RQWURO

During a test

Before starting a test

It is important to setup normal force control during any temperature change testing or curing testing Some general suggestions for normal force control For torsion testing, set normal force in tension: 1-2N ± 0.5-1.0N For curing or any parallel plate testing, set normal force in compression: 0 ± 0.5N

TAINSTRUMENTS.COM $56WUHVV5HOD[DWLRQ

Motor and transducer work in a feedback loop

TAINSTRUMENTS.COM $5&UHHS5HFRYHU\

Rule of thumb: recovery time is 2-3 times longer than creep time

TAINSTRUMENTS.COM $56WHDG\6WDWH$OJRULWKP&UHHS

Default values shown

During the test, the angular velocity is monitored with time to determine when stability has been reached. An average value for the angular velocity is recorded over the Sample period. When consecutive average values (Consecutive within tolerance) are within the tolerance specified here, the data is accepted.

TAINSTRUMENTS.COM $SSHQGL[5KHRPHWHU&DOLEUDWLRQV '+5DQG$5

TAINSTRUMENTS.COM '+5² &DOLEUDWLRQ2SWLRQV

Instrument Calibrations

Inertia (Service)

Rotational Mapping

Oscillation Mapping (recommended for interfacial measurements)

TAINSTRUMENTS.COM '+5² ,QHUWLD&DOLEUDWLRQ

Go to the Calibration tab and select Instrument

Make sure there is no geometry installed and then click calibrate

TAINSTRUMENTS.COM '+5² *HRPHWU\&DOLEUDWLRQ

Geometry Calibrations:

Inertia

Friction

Gap Temperature Compensation

Rotational Mapping

TAINSTRUMENTS.COM 7$7HFK7LS² *HRPHWU\&DOLEUDWLRQV

Videos available at www.tainstruments.com under the Videos tab or on the TA tech tip channel of YouTube™ (http://www.youtube.com/user/TATechTips)

TAINSTRUMENTS.COM 5KHRPHWHU&DOLEUDWLRQV $5(6*

TAINSTRUMENTS.COM $5(6*² &DOLEUDWLRQ2SWLRQV

Instrument Calibrations Temperature Offsets Phase Angle (Service) Measure Gap Temperature Compensation Transducer

Geometry Calibrations: Compliance and Inertia (from table) Gap Temperature Compensation

TAINSTRUMENTS.COM $5(6*² 7UDQVGXFHU&DOLEUDWLRQ

TAINSTRUMENTS.COM $5(6*² *HRPHWU\&DOLEUDWLRQ

Gap Temperature Compensation Enter manually or run calibration

Compliance and Inertia (from table in Help menu)

Geometry Constants Calculated based on dimensions

TAINSTRUMENTS.COM *HRPHWU\,QHUWLD &RPSOLDQFH +HOS0HQX

What if the online table does not list a compliance value for my specific geometry? Use the compliance value for a geometry of the same/similar dimension, type, and material.

TAINSTRUMENTS.COM $5(6* *DS7HPSHUDWXUH&RPSHQVDWLRQ

TAINSTRUMENTS.COM *HQHUDO5KHRPHWHU0DLQWHQDQFH

Air Supply Dry particulate-free air (dew point -40 °C) Check filters/regulators on a periodic basis to ensure proper pressure, free of moisture/oil/dirt buildup. If air must be turned off, then make sure that the bearing lock is fastened

NOTE: Do not rotate drive-shaft if air supply is OFF!

Location Isolate the instrument from vibrations with a marble table or Sorbathane pads. Drafts from fume hoods or HVAC systems and vibrations from adjacent equipment can contribute noise to measurements, particularly in the low torque regime. Use a Draft Shield to isolate instrument from drafts.

TAINSTRUMENTS.COM *HQHUDO5KHRPHWHU 0DLQWHQDQFH 3HOWLHU

Circulator Maintenance Proper operation of a fluid circulator is vital for correct and efficient operation of Peltier-based temperature control devices.

Check fluid levels and add anti-fungal additive regularly. Note: if operating circulator below 5°C then it is recommended to fill the circulator with a mixture or material with a lower freezing point than water to prevent permanent circulator damage. Example: add ~20% v/v ethanol to water Keep it clean!

Flush and clean circulator, Peltier system, and tubing at first sight of contamination.

When not in use, it is strongly recommended to deactivate the Peltier device and turn off the circulator.

TAINSTRUMENTS.COM *HRPHWU\,QIRUPDWLRQ² (VWLPDWHG0LQDQG0D[6KHDU5DWHV

Sample Max Shear Rate Min Shear Rate Geometry Diameter (mm) Degree Gap (micron) Volume (mL) (approx) 1/s (approx) 1/s 0 1000 0.05 1.20E+03 4.00E-07 0 500 0.03 8 0.5 18 1.17E-03 1 28 2.34E-03 2 52 4.68E-03 4 104 9.37E-03 0 1000 0.31 3.00E+03 1.00E-06 0.5 18 0.02 3.44E+04 1.15E-05 20 1280.041.72E+04 5.73E-06 2520.078.60E+03 2.87E-06 4 104 0.15 4.30E+03 1.43E-06 0 1000 0.49 3.75E+03 1.25E-06 Parallel Plate 0.5 18 0.04 and Cone and 25 1280.07 Plate 2520.14 4 104 0.29 0 1000 1.26 6.00E+03 2.00E-06 0.5 18 0.15 3.44E+04 1.15E-05 40 1280.291.72E+04 5.73E-06 2520.598.60E+03 2.87E-06 4 104 1.17 4.30E+03 1.43E-06 0 1000 2.83 9.00E+03 3.00E-06 0 500 1.41 60 0.5 18 0.49 3.44E+04 1.15E-05 1280.991.72E+04 5.73E-06 2521.978.60E+03 2.87E-06 4 104 3.95 4.30E+03 1.43E-06 Conical Din Rotor 19.6 4.36E+03 1.45E-06 Recessed End 6.65 4.36E+03 1.45E-06 Concentric Double Wall 11.65 1.59E+04 5.31E-06 Cylinder Pressure Cell 9.5 Standard Vane 28.72

TAINSTRUMENTS.COM %DVLF3DUDPHWHUVDQG8QLWV

^ƚƌĞƐƐс&ŽƌĐĞͬƌĞĂWĂ͕ŽƌĚǇŶĞͬĐŵϮ ʍсƐŚĞĂƌƐƚƌĞƐƐ ^ƚƌĂŝŶс'ĞŽŵĞƚƌŝĐ^ŚĂƉĞŚĂŶŐĞŶŽƵŶŝƚƐ γ сƐŚĞĂƌƐƚƌĂŝŶ ^ƚƌĂŝŶZĂƚĞŽƌ^ŚĞĂƌZĂƚĞсsĞůŽĐŝƚǇ'ƌĂĚŝĞŶƚϭͬƐ ɀሶ сƐŚĞĂƌƐƚƌĂŝŶƌĂƚĞ DŽĚƵůƵƐс^ƚƌĞƐƐͬ^ƚƌĂŝŶWĂŽƌĚǇŶĞͬĐŵϮ 'с^ŚĞĂƌDŽĚƵůƵƐ ŽŵƉůŝĂŶĐĞс^ƚƌĂŝŶͬ^ƚƌĞƐƐϭͬWĂŽƌĐŵϮͬĚǇŶĞ dǇƉŝĐĂůůǇĚĞŶŽƚĞĚďǇ: sŝƐĐŽƐŝƚǇс^ƚƌĞƐƐͬ^ƚƌĂŝŶZĂƚĞWĂͼƐ ŽƌWŽŝƐĞ ĞŶŽƚĞĚďǇη

^͘/͘ƵŶŝƚƐy ϭϬсĐ͘Ő͘Ɛ͘ƵŶŝƚƐ

TAINSTRUMENTS.COM &RPPRQ6\PEROVXVHGLQ5KHRORJ\

'ƌĞĞŬ >ĂƚŝŶ Ă ͗dĞŵƉĞƌĂƚƵƌĞƐŚŝĨƚĨĂĐƚŽƌ γ ;ŐĂŵŵĂͿ͗^ŚĞĂƌ^ƚƌĂŝŶ d ͗ƵůŬƌĞĞƉŽŵƉůŝĂŶĐĞ ߛሶ ;ŐĂŵŵĂĚŽƚͿ͗^ŚĞĂƌZĂƚĞ ͗dĞŶƐŝůĞŽŵƉůŝĂŶĐĞ δ ;ĚĞůƚĂͿ͗WŚĂƐĞŶŐůĞ ͗zŽƵŶŐ͛Ɛ;dĞŶƐŝůĞͿDŽĚƵůƵƐ ε ;ĞƉƐŝůŽŶͿ͗ůŽŶŐĂƚŝŽŶĂů ^ƚƌĂŝŶ ͛͗dĞŶƐŝůĞ^ƚŽƌĂŐĞDŽĚƵůƵƐ ݁ሶ ;ĞƉƐŝůŽŶĚŽƚͿ͗ůŽŶŐĂƚŝŽŶĂů ^ƚƌĂŝŶZĂƚĞ ͗͟dĞŶƐŝůĞ>ŽƐƐDŽĚƵůƵƐ η ;ĞƚĂͿ͗^ŚĞĂƌsŝƐĐŽƐŝƚǇ '͗^ŚĞĂƌDŽĚƵůƵƐ η ;ĞƚĂͿ͗ůŽŶŐĂƚŝŽŶĂů sŝƐĐŽƐŝƚǇ E '͛͗^ŚĞĂƌ^ƚŽƌĂŐĞDŽĚƵůƵƐ η* ;ĞƚĂƐƚĂƌͿ͗ ŽŵƉůĞǆsŝƐĐŽƐŝƚǇ '͗͟^ŚĞĂƌ>ŽƐƐDŽĚƵůƵƐ μ ;ŵƵͿ͗DŝĐƌŽŶƐ ΎŽƌ'Ύ͗ŽŵƉůĞǆDŽĚƵůƵƐ ν ;ŶƵͿ͗&ƌĞƋƵĞŶĐǇ;,ǌͿ :͗^ŚĞĂƌŽŵƉůŝĂŶĐĞ ρ ;ƌŚŽͿ͗ĞŶƐŝƚǇ <͗ƵůŬDŽĚƵůƵƐ;ŽƌĂůƐŽ^ƚŝĨĨŶĞƐƐͿ σ ;ƐŝŐŵĂͿ͗^ŚĞĂƌ^ƚƌĞƐƐ E ͗EŽƌŵĂů&ŽƌĐĞŝŶ^ƚĞĂĚǇ&ůŽǁ τ ;ƚĂƵͿ͗ůŽŶŐĂƚŝŽŶĂů ^ƚƌĞƐƐ ϭ d͗dĞŵƉĞƌĂƚƵƌĞ ω ;ŽŵĞŐĂͿ͗ŶŐƵůĂƌ &ƌĞƋƵĞŶĐǇ;ƌĂĚͬƐĞĐͿ dŐ͗'ůĂƐƐdƌĂŶƐŝƚŝŽŶdĞŵƉĞƌĂƚƵƌĞ

TAINSTRUMENTS.COM 6DPSOH3UHSDUDWLRQ 3RO\PHUV

TAINSTRUMENTS.COM .QRZ

Polymer samples come in different forms (e.g. powder, flakes, pellets) and can be sensitive to environmental conditions Careful sample preparation techniques are required to prepare good test specimens for reproducible testing

Molding a sample

Handling powders, flakes

Controling the environment

TAINSTRUMENTS.COM 0ROGLQJ3RO\PHU3HOOHWV

The best approach is to mold a sample plate (50x50 mm2 or 100x100 mm2) Molding temperature: 10 - 20°C > than test temperature Apply pressure: 8 – 12,000 lbs Keep at elevated temperature long enough to let the sample relax Cool down slowly under pressure to avoid orientations Punch out a sample disk (8 or 25 mm)

TAINSTRUMENTS.COM 0ROGLQJ3RZGHUVDQG)ODNHV

Before molding at high temperature, the sample has to be compacted cold to reduce the volume The compacted samples are transferred to the mold Follow steps from the molding pellets procedure Note: Sample may need to be stabilized or dried to avoid degradation

TAINSTRUMENTS.COM 3UHSDULQJ6HPLVROLG6DPSOHV

Cut rectangular sheets of prepreg or adhesive (30x30mm) Alternate direction of layer approx. 5 layer on top of each other (remove release paper from PSA) Compress the stack of sample layers in a press (4 – 5000 lbs) Punch out 25 mm disks

TAINSTRUMENTS.COM &RQWUROOLQJ(QYLURQPHQWDO&RQGLWLRQV'XULQJ6DPSOH3UHS

Polypropylene and Polyolefines in general tend to degrade fast – need to be stabilized by adding antioxidents Moisture sensitive materials such as polyamides and polyester require drying in vacuum or at temperatures around 80°C. Materials such as Polystyrene or Polymethyl- methacrylate (PMMA) also absorb moisture. In the melt phase, the gas separates into bubbles and the sample foams Pre-drying in vacuum is essential prior to testing Vacuum oven

TAINSTRUMENTS.COM /RDGLQJD0ROGHG'LVN

Geometry gap and Trim gap icons

Set Environmental System to test temperature

Load molded disk onto lower plate

Close the oven and Monitor Axial or After sample Close the oven and bring the upper Normal force relaxes, open the adjust gap to plate to the trim during this oven and trim geometry/test gap gap position period excess sample

TAINSTRUMENTS.COM /RDGLQJ3RO\PHU3HOOHW6DPSOHV

Set Environmental System to test temperature

Mount melt ring onto the lower plate and load pellets

Bring the upper After few minutes, After sample Close the oven and plate close to top of open the oven, relaxes, open the adjust gap to melt ring and close remove melt ring oven and trim geometry/test gap the oven and go to trim gap excess sample

TAINSTRUMENTS.COM 6DPSOH3UHSDUDWLRQ 6WUXFWXUHG)OXLGV

TAINSTRUMENTS.COM .QRZ

Structured fluids can range in consistency from low viscosity (e.g. milk) to high viscosity, pasty materials (e.g. tooth paste) Structured materials are very sensitive to mechnical and environmental conditions Be aware of largest particle size in sample and choose the geometry appropriately (cone vs parallel plate vs vane geometry) Samples can also be time dependent – how you treat the sample (handling, loading, pre-conditioning) may affect test results!

TAINSTRUMENTS.COM +DQGOLQJ/RZ9LVFRVLW\)OXLGV

Fluid samples which pour freely are relatively easy to handle prior to loading Keep the container closed to avoid evaporation of solvent or continuous phase Shake or stir sample to remove concentration gradients in suspensions Adequate shelf temperature may be necessary to avoid phase separation in emulsions Never return used sample into original flask to avoid contamination

TAINSTRUMENTS.COM /RDGLQJ/RZ9LVFRVLW\)OXLGV

Deposit fluid in the middle of the plate Set a motor velocity of ~ 1 rad/s and move to geometry gap Add additional material along the sides of the geometry – capillary forces will draw the sample between the gap When finished, click on the “Stop Motor” button NOTE: If the sample is a structured fluid, setting a motor velocity will introduce shear history onto the sample and can destroy the sample structure!

TAINSTRUMENTS.COM +DQGOLQJ3DVWH6OXUU\ *HO0DWHULDOV

The structure of high viscosity pastes and slurries may change with time Food samples, like dough, can change continuously The test samples need to be prepared carefully and consistently for each experiment to obtain reproducibility Slurries that may settle can gradually build a cake – these samples have to be tested before sedimentation

TAINSTRUMENTS.COM /RDGLQJ3DVWHVDQG6OXUULHV

Scoop up the paste with a spatula and deposit it at the center of the lower plate For less viscous materials, a syringe with a cut-off tip can be used Load ~ 10-20 excess material to ensure complete sample filling Set the gap to the trim gap and use exponential gap closure profile to minimize shear in the sample Lock the bearing, trim excess material and set final gap

TAINSTRUMENTS.COM +DQGOLQJ*HOV

Gels, especially chemical gels, may change irreversibly when large deformations are applied (for example, while loading) Prepare (formulate) the sample in the final shape required for the measurement so it can be loaded without deforming (cut, punch, …) Alternatively, prepare the sample in situ – on the rheometer Æ systemic rheology Take care to avoid introducing air bubbles!

TAINSTRUMENTS.COM